# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_a
_database_code_depnum_ccdc_archive 'CCDC 2169921'
loop_
_audit_author_name
_audit_author_address
'Jingcheng Feng'
;Technical Institution of Physics and Chemistry, Chinese Academy of Sciences
China
;
_audit_update_record             
;
2022-05-02 deposited with the CCDC.	2022-07-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'B4 K6 O12 Pr2'
_chemical_formula_weight         751.66

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_H-M_alt        'P n m a'
_space_group_name_Hall           '-P 2ac 2n'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   9.0940(12)
_cell_length_b                   7.1721(11)
_cell_length_c                   11.2310(16)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     732.52(18)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    2522
_cell_measurement_theta_min      2.88
_cell_measurement_theta_max      30.11

_exptl_crystal_description       Block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.408
_exptl_crystal_F_000             696
_exptl_transmission_factor_min   0.864
_exptl_transmission_factor_max   0.864
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_exptl_absorpt_coefficient_mu    8.332
_shelx_estimated_absorpt_T_min   0.435
_shelx_estimated_absorpt_T_max   0.555
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   sadabs
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            8219
_diffrn_reflns_av_unetI/netI     0.0695
_diffrn_reflns_av_R_equivalents  0.0929
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_theta_min         2.882
_diffrn_reflns_theta_max         30.516
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             1192
_reflns_number_gt                906
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0362P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         1192
_refine_ls_number_parameters     67
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0652
_refine_ls_R_factor_gt           0.0414
_refine_ls_wR_factor_ref         0.0866
_refine_ls_wR_factor_gt          0.0778
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_restrained_S_all      1.051
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
B1 B 0.5618(10) 0.7500 0.1245(8) 0.0098(18) Uani 1 2 d S T P . .
B2 B 0.5910(10) 0.7500 0.6181(8) 0.0098(19) Uani 1 2 d S T P . .
K1 K 0.4392(3) 0.7500 -0.1308(2) 0.0507(9) Uani 1 2 d S T P . .
K2 K 0.80019(14) 0.5033(2) -0.09768(11) 0.0173(3) Uani 1 1 d . . . . .
O1 O 0.6588(5) 0.7500 0.0319(5) 0.0155(14) Uani 1 2 d S T P . .
O2 O 0.6196(5) 0.7500 0.2397(5) 0.0159(14) Uani 1 2 d S T P . .
O3 O 0.4117(6) 0.7500 0.1127(5) 0.0166(14) Uani 1 2 d S T P . .
O4 O 0.5096(6) 0.7500 0.5135(5) 0.0118(12) Uani 1 2 d S T P . .
O5 O 0.6291(4) 0.9172(6) 0.6699(4) 0.0206(11) Uani 1 1 d . . . . .
Pr1 Pr 0.37379(5) 0.7500 0.33219(4) 0.00734(14) Uani 1 2 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
B1 O1 1.364(10) . ?
B1 O3 1.372(11) . ?
B1 O2 1.397(10) . ?
B1 Pr1 2.878(9) 6_656 ?
B1 Pr1 2.892(9) . ?
B1 K1 3.077(9) . ?
B1 K1 3.5868(6) 5_665 ?
B1 K1 3.5868(6) 5_675 ?
B2 O5 1.378(6) 7_575 ?
B2 O5 1.378(6) . ?
B2 O4 1.389(10) . ?
B2 K1 3.140(9) 1_556 ?
B2 K1 3.170(9) 6_656 ?
B2 K2 3.187(7) 2_665 ?
B2 K2 3.187(7) 8_766 ?
B2 K2 3.190(8) 6_556 ?
B2 K2 3.190(8) 4_465 ?
K1 O1 2.707(6) . ?
K1 O3 2.747(6) . ?
K1 O5 3.071(5) 7_574 ?
K1 O5 3.071(5) 1_554 ?
K1 O5 3.095(4) 4_465 ?
K1 O5 3.095(4) 6_556 ?
K1 B2 3.140(9) 1_554 ?
K1 B2 3.170(9) 6_556 ?
K1 B1 3.5868(6) 5_675 ?
K1 B1 3.5868(6) 5_665 ?
K1 K2 3.745(2) 6 ?
K2 O1 2.627(4) . ?
K2 O3 2.654(4) 5_665 ?
K2 O2 2.677(4) 2_664 ?
K2 O4 2.766(4) 6_656 ?
K2 O4 2.802(4) 2_664 ?
K2 O5 3.091(4) 7_574 ?
K2 O5 3.135(4) 8_755 ?
K2 O5 3.152(4) 4_565 ?
K2 B2 3.187(7) 2_664 ?
K2 B2 3.190(8) 6_656 ?
K2 Pr1 3.5311(13) 6_656 ?
K2 K2 3.539(3) 7_575 ?
O1 Pr1 2.481(5) 6_656 ?
O1 K2 2.627(4) 7_575 ?
O2 Pr1 2.448(5) 6_656 ?
O2 Pr1 2.465(5) . ?
O2 K2 2.677(4) 8_766 ?
O2 K2 2.677(4) 2_665 ?
O3 Pr1 2.489(6) . ?
O3 K2 2.654(4) 5_665 ?
O3 K2 2.654(4) 3_655 ?
O4 Pr1 2.381(5) . ?
O4 K2 2.766(4) 6_556 ?
O4 K2 2.766(4) 4_465 ?
O4 K2 2.802(4) 8_766 ?
O4 K2 2.802(4) 2_665 ?
O5 Pr1 2.387(4) 5_676 ?
O5 K1 3.071(5) 1_556 ?
O5 K2 3.091(4) 7_576 ?
O5 K1 3.095(4) 6_656 ?
O5 K2 3.135(4) 8_766 ?
O5 K2 3.152(4) 4_465 ?
Pr1 O5 2.387(4) 3_646 ?
Pr1 O5 2.387(4) 5_676 ?
Pr1 O2 2.448(5) 6_556 ?
Pr1 O1 2.481(5) 6_556 ?
Pr1 B1 2.878(9) 6_556 ?
Pr1 K2 3.5311(13) 4_465 ?
Pr1 K2 3.5311(13) 6_556 ?
Pr1 K2 3.5653(14) 8_766 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 B1 O3 124.7(8) . . ?
O1 B1 O2 117.6(7) . . ?
O3 B1 O2 117.7(7) . . ?
O1 B1 Pr1 59.4(4) . 6_656 ?
O3 B1 Pr1 175.8(6) . 6_656 ?
O2 B1 Pr1 58.2(4) . 6_656 ?
O1 B1 Pr1 176.0(6) . . ?
O3 B1 Pr1 59.3(4) . . ?
O2 B1 Pr1 58.4(4) . . ?
Pr1 B1 Pr1 116.5(3) 6_656 . ?
O1 B1 K1 61.5(4) . . ?
O3 B1 K1 63.2(4) . . ?
O2 B1 K1 179.1(6) . . ?
Pr1 B1 K1 121.0(3) 6_656 . ?
Pr1 B1 K1 122.5(3) . . ?
O1 B1 K1 90.95(15) . 5_665 ?
O3 B1 K1 89.97(16) . 5_665 ?
O2 B1 K1 89.01(15) . 5_665 ?
Pr1 B1 K1 89.95(15) 6_656 5_665 ?
Pr1 B1 K1 89.00(15) . 5_665 ?
K1 B1 K1 91.00(15) . 5_665 ?
O1 B1 K1 90.95(15) . 5_675 ?
O3 B1 K1 89.97(16) . 5_675 ?
O2 B1 K1 89.01(15) . 5_675 ?
Pr1 B1 K1 89.95(15) 6_656 5_675 ?
Pr1 B1 K1 89.00(15) . 5_675 ?
K1 B1 K1 91.00(15) . 5_675 ?
K1 B1 K1 177.7(3) 5_665 5_675 ?
O5 B2 O5 121.1(7) 7_575 . ?
O5 B2 O4 119.5(4) 7_575 . ?
O5 B2 O4 119.5(4) . . ?
O5 B2 K1 74.4(4) 7_575 1_556 ?
O5 B2 K1 74.4(4) . 1_556 ?
O4 B2 K1 121.7(5) . 1_556 ?
O5 B2 K1 74.3(4) 7_575 6_656 ?
O5 B2 K1 74.3(4) . 6_656 ?
O4 B2 K1 124.8(5) . 6_656 ?
K1 B2 K1 113.5(3) 1_556 6_656 ?
O5 B2 K2 75.3(3) 7_575 2_665 ?
O5 B2 K2 137.7(5) . 2_665 ?
O4 B2 K2 61.4(3) . 2_665 ?
K1 B2 K2 145.05(9) 1_556 2_665 ?
K1 B2 K2 73.98(18) 6_656 2_665 ?
O5 B2 K2 137.7(5) 7_575 8_766 ?
O5 B2 K2 75.3(3) . 8_766 ?
O4 B2 K2 61.4(3) . 8_766 ?
K1 B2 K2 145.05(9) 1_556 8_766 ?
K1 B2 K2 73.98(18) 6_656 8_766 ?
K2 B2 K2 69.52(18) 2_665 8_766 ?
O5 B2 K2 75.9(3) 7_575 6_556 ?
O5 B2 K2 136.2(5) . 6_556 ?
O4 B2 K2 59.8(3) . 6_556 ?
K1 B2 K2 72.55(18) 1_556 6_556 ?
K1 B2 K2 146.24(9) 6_656 6_556 ?
K2 B2 K2 83.48(15) 2_665 6_556 ?
K2 B2 K2 121.3(3) 8_766 6_556 ?
O5 B2 K2 136.2(5) 7_575 4_465 ?
O5 B2 K2 75.9(3) . 4_465 ?
O4 B2 K2 59.8(3) . 4_465 ?
K1 B2 K2 72.55(18) 1_556 4_465 ?
K1 B2 K2 146.24(9) 6_656 4_465 ?
K2 B2 K2 121.3(3) 2_665 4_465 ?
K2 B2 K2 83.48(15) 8_766 4_465 ?
K2 B2 K2 67.37(18) 6_556 4_465 ?
O1 K1 O3 52.76(16) . . ?
O1 K1 O5 94.41(14) . 7_574 ?
O3 K1 O5 140.97(13) . 7_574 ?
O1 K1 O5 94.41(14) . 1_554 ?
O3 K1 O5 140.97(13) . 1_554 ?
O5 K1 O5 45.98(16) 7_574 1_554 ?
O1 K1 B1 26.3(2) . . ?
O3 K1 B1 26.5(2) . . ?
O5 K1 B1 118.37(18) 7_574 . ?
O5 K1 B1 118.37(18) 1_554 . ?
O1 K1 O5 140.16(14) . 4_465 ?
O3 K1 O5 93.35(14) . 4_465 ?
O5 K1 O5 104.93(11) 7_574 4_465 ?
O5 K1 O5 124.08(10) 1_554 4_465 ?
B1 K1 O5 117.55(18) . 4_465 ?
O1 K1 O5 140.16(14) . 6_556 ?
O3 K1 O5 93.35(14) . 6_556 ?
O5 K1 O5 124.08(10) 7_574 6_556 ?
O5 K1 O5 104.93(11) 1_554 6_556 ?
B1 K1 O5 117.55(18) . 6_556 ?
O5 K1 O5 45.60(16) 4_465 6_556 ?
O1 K1 B2 106.4(2) . 1_554 ?
O3 K1 B2 159.1(2) . 1_554 ?
O5 K1 B2 25.60(11) 7_574 1_554 ?
O5 K1 B2 25.60(11) 1_554 1_554 ?
B1 K1 B2 132.7(2) . 1_554 ?
O5 K1 B2 105.84(18) 4_465 1_554 ?
O5 K1 B2 105.84(18) 6_556 1_554 ?
O1 K1 B2 135.0(2) . 6_556 ?
O3 K1 B2 82.2(2) . 6_556 ?
O5 K1 B2 126.50(17) 7_574 6_556 ?
O5 K1 B2 126.50(17) 1_554 6_556 ?
B1 K1 B2 108.7(2) . 6_556 ?
O5 K1 B2 25.37(10) 4_465 6_556 ?
O5 K1 B2 25.37(10) 6_556 6_556 ?
B2 K1 B2 118.67(18) 1_554 6_556 ?
O1 K1 B1 89.35(15) . 5_675 ?
O3 K1 B1 88.86(15) . 5_675 ?
O5 K1 B1 113.97(18) 7_574 5_675 ?
O5 K1 B1 67.99(17) 1_554 5_675 ?
B1 K1 B1 89.00(15) . 5_675 ?
O5 K1 B1 112.83(18) 4_465 5_675 ?
O5 K1 B1 67.24(17) 6_556 5_675 ?
B2 K1 B1 91.08(15) 1_554 5_675 ?
B2 K1 B1 89.80(16) 6_556 5_675 ?
O1 K1 B1 89.35(15) . 5_665 ?
O3 K1 B1 88.86(15) . 5_665 ?
O5 K1 B1 67.99(17) 7_574 5_665 ?
O5 K1 B1 113.97(18) 1_554 5_665 ?
B1 K1 B1 89.00(15) . 5_665 ?
O5 K1 B1 67.24(17) 4_465 5_665 ?
O5 K1 B1 112.83(18) 6_556 5_665 ?
B2 K1 B1 91.08(15) 1_554 5_665 ?
B2 K1 B1 89.80(16) 6_556 5_665 ?
B1 K1 B1 177.7(3) 5_675 5_665 ?
O1 K1 K2 143.00(9) . 6 ?
O3 K1 K2 141.27(9) . 6 ?
O5 K1 K2 53.99(8) 7_574 6 ?
O5 K1 K2 77.36(9) 1_554 6 ?
B1 K1 K2 151.78(3) . 6 ?
O5 K1 K2 52.70(8) 4_465 6 ?
O5 K1 K2 76.12(9) 6_556 6 ?
B2 K1 K2 54.35(14) 1_554 6 ?
B2 K1 K2 72.51(15) 6_556 6 ?
B1 K1 K2 119.18(16) 5_675 6 ?
B1 K1 K2 62.80(15) 5_665 6 ?
O1 K2 O3 98.10(13) . 5_665 ?
O1 K2 O2 165.51(16) . 2_664 ?
O3 K2 O2 71.92(14) 5_665 2_664 ?
O1 K2 O4 73.56(14) . 6_656 ?
O3 K2 O4 163.65(16) 5_665 6_656 ?
O2 K2 O4 118.67(14) 2_664 6_656 ?
O1 K2 O4 119.47(15) . 2_664 ?
O3 K2 O4 91.87(12) 5_665 2_664 ?
O2 K2 O4 72.28(14) 2_664 2_664 ?
O4 K2 O4 80.64(4) 6_656 2_664 ?
O1 K2 O5 95.58(14) . 7_574 ?
O3 K2 O5 72.97(13) 5_665 7_574 ?
O2 K2 O5 71.72(13) 2_664 7_574 ?
O4 K2 O5 121.15(13) 6_656 7_574 ?
O4 K2 O5 143.74(13) 2_664 7_574 ?
O1 K2 O5 72.65(13) . 8_755 ?
O3 K2 O5 94.30(14) 5_665 8_755 ?
O2 K2 O5 117.67(13) 2_664 8_755 ?
O4 K2 O5 69.94(13) 6_656 8_755 ?
O4 K2 O5 47.05(12) 2_664 8_755 ?
O5 K2 O5 161.60(7) 7_574 8_755 ?
O1 K2 O5 119.05(13) . 4_565 ?
O3 K2 O5 142.81(13) 5_665 4_565 ?
O2 K2 O5 71.85(12) 2_664 4_565 ?
O4 K2 O5 47.07(13) 6_656 4_565 ?
O4 K2 O5 69.27(12) 2_664 4_565 ?
O5 K2 O5 103.12(7) 7_574 4_565 ?
O5 K2 O5 95.04(10) 8_755 4_565 ?
O1 K2 B2 96.58(17) . 2_664 ?
O3 K2 B2 83.31(16) 5_665 2_664 ?
O2 K2 B2 92.71(16) 2_664 2_664 ?
O4 K2 B2 83.73(14) 6_656 2_664 ?
O4 K2 B2 25.80(18) 2_664 2_664 ?
O5 K2 B2 154.62(13) 7_574 2_664 ?
O5 K2 B2 25.16(13) 8_755 2_664 ?
O5 K2 B2 90.24(18) 4_565 2_664 ?
O1 K2 B2 94.14(15) . 6_656 ?
O3 K2 B2 167.71(17) 5_665 6_656 ?
O2 K2 B2 95.83(16) 2_664 6_656 ?
O4 K2 B2 25.72(18) 6_656 6_656 ?
O4 K2 B2 83.11(14) 2_664 6_656 ?
O5 K2 B2 104.73(17) 7_574 6_656 ?
O5 K2 B2 90.47(18) 8_755 6_656 ?
O5 K2 B2 25.09(13) 4_565 6_656 ?
B2 K2 B2 96.51(15) 2_664 6_656 ?
O1 K2 Pr1 44.57(11) . 6_656 ?
O3 K2 Pr1 122.30(13) 5_665 6_656 ?
O2 K2 Pr1 149.81(11) 2_664 6_656 ?
O4 K2 Pr1 42.30(11) 6_656 6_656 ?
O4 K2 Pr1 80.31(9) 2_664 6_656 ?
O5 K2 Pr1 135.72(9) 7_574 6_656 ?
O5 K2 Pr1 41.43(8) 8_755 6_656 ?
O5 K2 Pr1 86.96(8) 4_565 6_656 ?
B2 K2 Pr1 65.45(10) 2_664 6_656 ?
B2 K2 Pr1 68.02(16) 6_656 6_656 ?
O1 K2 K2 47.67(8) . 7_575 ?
O3 K2 K2 133.21(8) 5_665 7_575 ?
O2 K2 K2 132.74(8) 2_664 7_575 ?
O4 K2 K2 50.24(8) 6_656 7_575 ?
O4 K2 K2 130.42(8) 2_664 7_575 ?
O5 K2 K2 79.38(8) 7_574 7_575 ?
O5 K2 K2 101.36(8) 8_755 7_575 ?
O5 K2 K2 79.58(8) 4_565 7_575 ?
B2 K2 K2 124.76(9) 2_664 7_575 ?
B2 K2 K2 56.31(9) 6_656 7_575 ?
Pr1 K2 K2 59.93(2) 6_656 7_575 ?
B1 O1 Pr1 92.3(5) . 6_656 ?
B1 O1 K2 137.65(8) . 7_575 ?
Pr1 O1 K2 87.42(14) 6_656 7_575 ?
B1 O1 K2 137.65(8) . . ?
Pr1 O1 K2 87.42(14) 6_656 . ?
K2 O1 K2 84.67(16) 7_575 . ?
B1 O1 K1 92.2(5) . . ?
Pr1 O1 K1 175.5(2) 6_656 . ?
K2 O1 K1 89.26(15) 7_575 . ?
K2 O1 K1 89.26(15) . . ?
B1 O2 Pr1 92.8(5) . 6_656 ?
B1 O2 Pr1 92.8(4) . . ?
Pr1 O2 Pr1 174.4(2) 6_656 . ?
B1 O2 K2 137.26(8) . 8_766 ?
Pr1 O2 K2 88.16(13) 6_656 8_766 ?
Pr1 O2 K2 87.69(14) . 8_766 ?
B1 O2 K2 137.26(8) . 2_665 ?
Pr1 O2 K2 88.16(13) 6_656 2_665 ?
Pr1 O2 K2 87.69(14) . 2_665 ?
K2 O2 K2 85.48(16) 8_766 2_665 ?
B1 O3 Pr1 92.4(5) . . ?
B1 O3 K2 136.79(8) . 5_665 ?
Pr1 O3 K2 87.85(15) . 5_665 ?
B1 O3 K2 136.79(8) . 3_655 ?
Pr1 O3 K2 87.85(15) . 3_655 ?
K2 O3 K2 86.41(17) 5_665 3_655 ?
B1 O3 K1 90.3(5) . . ?
Pr1 O3 K1 177.3(2) . . ?
K2 O3 K1 90.15(15) 5_665 . ?
K2 O3 K1 90.15(15) 3_655 . ?
B2 O4 Pr1 179.1(5) . . ?
B2 O4 K2 94.4(3) . 6_556 ?
Pr1 O4 K2 86.28(14) . 6_556 ?
B2 O4 K2 94.4(3) . 4_465 ?
Pr1 O4 K2 86.28(14) . 4_465 ?
K2 O4 K2 79.52(15) 6_556 4_465 ?
B2 O4 K2 92.8(3) . 8_766 ?
Pr1 O4 K2 86.52(15) . 8_766 ?
K2 O4 K2 172.8(2) 6_556 8_766 ?
K2 O4 K2 99.36(4) 4_465 8_766 ?
B2 O4 K2 92.8(3) . 2_665 ?
Pr1 O4 K2 86.52(15) . 2_665 ?
K2 O4 K2 99.36(4) 6_556 2_665 ?
K2 O4 K2 172.8(2) 4_465 2_665 ?
K2 O4 K2 80.85(15) 8_766 2_665 ?
B2 O5 Pr1 149.7(4) . 5_676 ?
B2 O5 K1 80.0(4) . 1_556 ?
Pr1 O5 K1 113.05(15) 5_676 1_556 ?
B2 O5 K2 130.1(4) . 7_576 ?
Pr1 O5 K2 80.20(12) 5_676 7_576 ?
K1 O5 K2 74.92(10) 1_556 7_576 ?
B2 O5 K1 80.3(4) . 6_656 ?
Pr1 O5 K1 113.34(14) 5_676 6_656 ?
K1 O5 K1 117.68(14) 1_556 6_656 ?
K2 O5 K1 74.51(9) 7_576 6_656 ?
B2 O5 K2 79.5(4) . 8_766 ?
Pr1 O5 K2 78.21(12) 5_676 8_766 ?
K1 O5 K2 152.98(14) 1_556 8_766 ?
K2 O5 K2 132.07(13) 7_576 8_766 ?
K1 O5 K2 75.73(11) 6_656 8_766 ?
B2 O5 K2 79.0(4) . 4_465 ?
Pr1 O5 K2 78.82(11) 5_676 4_465 ?
K1 O5 K2 73.99(10) 1_556 4_465 ?
K2 O5 K2 131.43(14) 7_576 4_465 ?
K1 O5 K2 153.91(15) 6_656 4_465 ?
K2 O5 K2 84.96(10) 8_766 4_465 ?
O4 Pr1 O5 90.82(9) . 3_646 ?
O4 Pr1 O5 90.82(9) . 5_676 ?
O5 Pr1 O5 178.28(18) 3_646 5_676 ?
O4 Pr1 O2 140.52(18) . 6_556 ?
O5 Pr1 O2 89.20(9) 3_646 6_556 ?
O5 Pr1 O2 89.20(9) 5_676 6_556 ?
O4 Pr1 O2 83.66(18) . . ?
O5 Pr1 O2 90.34(10) 3_646 . ?
O5 Pr1 O2 90.34(10) 5_676 . ?
O2 Pr1 O2 135.82(2) 6_556 . ?
O4 Pr1 O1 83.27(17) . 6_556 ?
O5 Pr1 O1 89.85(10) 3_646 6_556 ?
O5 Pr1 O1 89.85(10) 5_676 6_556 ?
O2 Pr1 O1 57.25(16) 6_556 6_556 ?
O2 Pr1 O1 166.93(16) . 6_556 ?
O4 Pr1 O3 140.79(17) . . ?
O5 Pr1 O3 89.52(10) 3_646 . ?
O5 Pr1 O3 89.52(10) 5_676 . ?
O2 Pr1 O3 78.69(18) 6_556 . ?
O2 Pr1 O3 57.13(17) . . ?
O1 Pr1 O3 135.94(18) 6_556 . ?
O4 Pr1 B1 111.5(2) . 6_556 ?
O5 Pr1 B1 89.47(10) 3_646 6_556 ?
O5 Pr1 B1 89.47(10) 5_676 6_556 ?
O2 Pr1 B1 29.0(2) 6_556 6_556 ?
O2 Pr1 B1 164.8(2) . 6_556 ?
O1 Pr1 B1 28.3(2) 6_556 6_556 ?
O3 Pr1 B1 107.7(2) . 6_556 ?
O4 Pr1 B1 112.5(2) . . ?
O5 Pr1 B1 89.92(10) 3_646 . ?
O5 Pr1 B1 89.92(10) 5_676 . ?
O2 Pr1 B1 107.0(2) 6_556 . ?
O2 Pr1 B1 28.8(2) . . ?
O1 Pr1 B1 164.2(2) 6_556 . ?
O3 Pr1 B1 28.3(2) . . ?
B1 Pr1 B1 136.0(2) 6_556 . ?
O4 Pr1 K2 51.42(10) . 4_465 ?
O5 Pr1 K2 120.49(10) 3_646 4_465 ?
O5 Pr1 K2 60.35(10) 5_676 4_465 ?
O2 Pr1 K2 95.72(11) 6_556 4_465 ?
O2 Pr1 K2 121.84(10) . 4_465 ?
O1 Pr1 K2 48.01(9) 6_556 4_465 ?
O3 Pr1 K2 149.60(3) . 4_465 ?
B1 Pr1 K2 70.77(15) 6_556 4_465 ?
B1 Pr1 K2 142.47(11) . 4_465 ?
O4 Pr1 K2 51.42(10) . 6_556 ?
O5 Pr1 K2 60.35(10) 3_646 6_556 ?
O5 Pr1 K2 120.49(10) 5_676 6_556 ?
O2 Pr1 K2 95.72(11) 6_556 6_556 ?
O2 Pr1 K2 121.84(10) . 6_556 ?
O1 Pr1 K2 48.01(9) 6_556 6_556 ?
O3 Pr1 K2 149.60(3) . 6_556 ?
B1 Pr1 K2 70.77(15) 6_556 6_556 ?
B1 Pr1 K2 142.47(11) . 6_556 ?
K2 Pr1 K2 60.14(5) 4_465 6_556 ?
O4 Pr1 K2 51.66(10) . 8_766 ?
O5 Pr1 K2 121.40(10) 3_646 8_766 ?
O5 Pr1 K2 60.13(9) 5_676 8_766 ?
O2 Pr1 K2 149.08(3) 6_556 8_766 ?
O2 Pr1 K2 48.61(9) . 8_766 ?
O1 Pr1 K2 121.30(10) 6_556 8_766 ?
O3 Pr1 K2 95.95(11) . 8_766 ?
B1 Pr1 K2 141.47(10) 6_556 8_766 ?
B1 Pr1 K2 71.73(15) . 8_766 ?
K2 Pr1 K2 73.49(3) 4_465 8_766 ?
K2 Pr1 K2 103.09(2) 6_556 8_766 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O3 B1 O1 Pr1 180.000(0) . . . 6_656 ?
O2 B1 O1 Pr1 0.000(1) . . . 6_656 ?
K1 B1 O1 Pr1 180.000(0) . . . 6_656 ?
K1 B1 O1 Pr1 -89.38(16) 5_665 . . 6_656 ?
K1 B1 O1 Pr1 89.38(16) 5_675 . . 6_656 ?
O3 B1 O1 K2 91.3(6) . . . 7_575 ?
O2 B1 O1 K2 -88.7(6) . . . 7_575 ?
Pr1 B1 O1 K2 -88.7(6) 6_656 . . 7_575 ?
K1 B1 O1 K2 91.3(6) . . . 7_575 ?
K1 B1 O1 K2 -178.1(5) 5_665 . . 7_575 ?
K1 B1 O1 K2 0.7(7) 5_675 . . 7_575 ?
O3 B1 O1 K2 -91.3(6) . . . . ?
O2 B1 O1 K2 88.7(6) . . . . ?
Pr1 B1 O1 K2 88.7(6) 6_656 . . . ?
K1 B1 O1 K2 -91.3(6) . . . . ?
K1 B1 O1 K2 -0.7(7) 5_665 . . . ?
K1 B1 O1 K2 178.1(5) 5_675 . . . ?
O3 B1 O1 K1 0.000(0) . . . . ?
O2 B1 O1 K1 180.000(1) . . . . ?
Pr1 B1 O1 K1 180.000(0) 6_656 . . . ?
K1 B1 O1 K1 90.62(16) 5_665 . . . ?
K1 B1 O1 K1 -90.62(16) 5_675 . . . ?
O1 B1 O2 Pr1 0.000(0) . . . 6_656 ?
O3 B1 O2 Pr1 180.000(0) . . . 6_656 ?
Pr1 B1 O2 Pr1 180.000(0) . . . 6_656 ?
K1 B1 O2 Pr1 90.56(15) 5_665 . . 6_656 ?
K1 B1 O2 Pr1 -90.56(15) 5_675 . . 6_656 ?
O1 B1 O2 Pr1 180.000(0) . . . . ?
O3 B1 O2 Pr1 0.000(0) . . . . ?
Pr1 B1 O2 Pr1 180.000(0) 6_656 . . . ?
K1 B1 O2 Pr1 -89.44(15) 5_665 . . . ?
K1 B1 O2 Pr1 89.44(15) 5_675 . . . ?
O1 B1 O2 K2 90.4(5) . . . 8_766 ?
O3 B1 O2 K2 -89.6(5) . . . 8_766 ?
Pr1 B1 O2 K2 90.4(5) 6_656 . . 8_766 ?
Pr1 B1 O2 K2 -89.6(5) . . . 8_766 ?
K1 B1 O2 K2 -179.1(4) 5_665 . . 8_766 ?
K1 B1 O2 K2 -0.2(7) 5_675 . . 8_766 ?
O1 B1 O2 K2 -90.4(5) . . . 2_665 ?
O3 B1 O2 K2 89.6(5) . . . 2_665 ?
Pr1 B1 O2 K2 -90.4(5) 6_656 . . 2_665 ?
Pr1 B1 O2 K2 89.6(5) . . . 2_665 ?
K1 B1 O2 K2 0.2(7) 5_665 . . 2_665 ?
K1 B1 O2 K2 179.1(4) 5_675 . . 2_665 ?
O1 B1 O3 Pr1 180.000(0) . . . . ?
O2 B1 O3 Pr1 0.000(1) . . . . ?
K1 B1 O3 Pr1 180.0 . . . . ?
K1 B1 O3 Pr1 88.86(15) 5_665 . . . ?
K1 B1 O3 Pr1 -88.86(15) 5_675 . . . ?
O1 B1 O3 K2 90.6(6) . . . 5_665 ?
O2 B1 O3 K2 -89.4(6) . . . 5_665 ?
Pr1 B1 O3 K2 -89.4(6) . . . 5_665 ?
K1 B1 O3 K2 90.6(6) . . . 5_665 ?
K1 B1 O3 K2 -0.6(7) 5_665 . . 5_665 ?
K1 B1 O3 K2 -178.3(5) 5_675 . . 5_665 ?
O1 B1 O3 K2 -90.6(6) . . . 3_655 ?
O2 B1 O3 K2 89.4(6) . . . 3_655 ?
Pr1 B1 O3 K2 89.4(6) . . . 3_655 ?
K1 B1 O3 K2 -90.6(6) . . . 3_655 ?
K1 B1 O3 K2 178.3(5) 5_665 . . 3_655 ?
K1 B1 O3 K2 0.6(7) 5_675 . . 3_655 ?
O1 B1 O3 K1 0.000(0) . . . . ?
O2 B1 O3 K1 180.000(1) . . . . ?
Pr1 B1 O3 K1 180.000(1) . . . . ?
K1 B1 O3 K1 -91.14(15) 5_665 . . . ?
K1 B1 O3 K1 91.14(15) 5_675 . . . ?
O5 B2 O4 K2 49.3(7) 7_575 . . 6_556 ?
O5 B2 O4 K2 -129.1(6) . . . 6_556 ?
K1 B2 O4 K2 -39.90(9) 1_556 . . 6_556 ?
K1 B2 O4 K2 140.10(9) 6_656 . . 6_556 ?
K2 B2 O4 K2 99.62(4) 2_665 . . 6_556 ?
K2 B2 O4 K2 -179.42(17) 8_766 . . 6_556 ?
K2 B2 O4 K2 -79.80(18) 4_465 . . 6_556 ?
O5 B2 O4 K2 129.1(6) 7_575 . . 4_465 ?
O5 B2 O4 K2 -49.3(7) . . . 4_465 ?
K1 B2 O4 K2 39.90(9) 1_556 . . 4_465 ?
K1 B2 O4 K2 -140.10(9) 6_656 . . 4_465 ?
K2 B2 O4 K2 179.42(17) 2_665 . . 4_465 ?
K2 B2 O4 K2 -99.62(4) 8_766 . . 4_465 ?
K2 B2 O4 K2 79.80(18) 6_556 . . 4_465 ?
O5 B2 O4 K2 -131.3(6) 7_575 . . 8_766 ?
O5 B2 O4 K2 50.3(7) . . . 8_766 ?
K1 B2 O4 K2 139.52(8) 1_556 . . 8_766 ?
K1 B2 O4 K2 -40.48(8) 6_656 . . 8_766 ?
K2 B2 O4 K2 -80.96(16) 2_665 . . 8_766 ?
K2 B2 O4 K2 179.42(17) 6_556 . . 8_766 ?
K2 B2 O4 K2 99.62(4) 4_465 . . 8_766 ?
O5 B2 O4 K2 -50.3(7) 7_575 . . 2_665 ?
O5 B2 O4 K2 131.3(6) . . . 2_665 ?
K1 B2 O4 K2 -139.52(8) 1_556 . . 2_665 ?
K1 B2 O4 K2 40.48(8) 6_656 . . 2_665 ?
K2 B2 O4 K2 80.96(16) 8_766 . . 2_665 ?
K2 B2 O4 K2 -99.62(4) 6_556 . . 2_665 ?
K2 B2 O4 K2 -179.42(17) 4_465 . . 2_665 ?
O5 B2 O5 Pr1 -179.50(19) 7_575 . . 5_676 ?
O4 B2 O5 Pr1 -1.1(14) . . . 5_676 ?
K1 B2 O5 Pr1 -119.1(8) 1_556 . . 5_676 ?
K1 B2 O5 Pr1 120.3(8) 6_656 . . 5_676 ?
K2 B2 O5 Pr1 77.6(11) 2_665 . . 5_676 ?
K2 B2 O5 Pr1 43.2(8) 8_766 . . 5_676 ?
K2 B2 O5 Pr1 -76.9(11) 6_556 . . 5_676 ?
K2 B2 O5 Pr1 -43.6(8) 4_465 . . 5_676 ?
O5 B2 O5 K1 -60.4(7) 7_575 . . 1_556 ?
O4 B2 O5 K1 118.0(7) . . . 1_556 ?
K1 B2 O5 K1 -120.57(14) 6_656 . . 1_556 ?
K2 B2 O5 K1 -163.3(7) 2_665 . . 1_556 ?
K2 B2 O5 K1 162.30(15) 8_766 . . 1_556 ?
K2 B2 O5 K1 42.2(6) 6_556 . . 1_556 ?
K2 B2 O5 K1 75.47(10) 4_465 . . 1_556 ?
O5 B2 O5 K2 0.0(11) 7_575 . . 7_576 ?
O4 B2 O5 K2 178.4(4) . . . 7_576 ?
K1 B2 O5 K2 60.4(4) 1_556 . . 7_576 ?
K1 B2 O5 K2 -60.2(4) 6_656 . . 7_576 ?
K2 B2 O5 K2 -102.9(7) 2_665 . . 7_576 ?
K2 B2 O5 K2 -137.3(4) 8_766 . . 7_576 ?
K2 B2 O5 K2 102.6(6) 6_556 . . 7_576 ?
K2 B2 O5 K2 135.9(4) 4_465 . . 7_576 ?
O5 B2 O5 K1 60.2(7) 7_575 . . 6_656 ?
O4 B2 O5 K1 -121.4(7) . . . 6_656 ?
K1 B2 O5 K1 120.57(14) 1_556 . . 6_656 ?
K2 B2 O5 K1 -42.7(6) 2_665 . . 6_656 ?
K2 B2 O5 K1 -77.13(11) 8_766 . . 6_656 ?
K2 B2 O5 K1 162.7(6) 6_556 . . 6_656 ?
K2 B2 O5 K1 -163.97(16) 4_465 . . 6_656 ?
O5 B2 O5 K2 137.3(8) 7_575 . . 8_766 ?
O4 B2 O5 K2 -44.3(6) . . . 8_766 ?
K1 B2 O5 K2 -162.30(15) 1_556 . . 8_766 ?
K1 B2 O5 K2 77.13(10) 6_656 . . 8_766 ?
K2 B2 O5 K2 34.4(6) 2_665 . . 8_766 ?
K2 B2 O5 K2 -120.1(6) 6_556 . . 8_766 ?
K2 B2 O5 K2 -86.84(11) 4_465 . . 8_766 ?
O5 B2 O5 K2 -135.9(8) 7_575 . . 4_465 ?
O4 B2 O5 K2 42.5(6) . . . 4_465 ?
K1 B2 O5 K2 -75.47(10) 1_556 . . 4_465 ?
K1 B2 O5 K2 163.97(16) 6_656 . . 4_465 ?
K2 B2 O5 K2 121.3(7) 2_665 . . 4_465 ?
K2 B2 O5 K2 86.84(11) 8_766 . . 4_465 ?
K2 B2 O5 K2 -33.3(5) 6_556 . . 4_465 ?

_refine_diff_density_max         1.512
_refine_diff_density_min         -2.018
_refine_diff_density_rms         0.370



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_a_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 2169922'
loop_
_audit_author_name
_audit_author_address
'Jingcheng Feng'
;Technical Institution of Physics and Chemistry, Chinese Academy of Sciences
China
;
_audit_update_record             
;
2022-05-02 deposited with the CCDC.	2022-07-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'B4 K6 Nd2 O12'
_chemical_formula_weight         758.32

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_H-M_alt        'P n m a'
_space_group_name_Hall           '-P 2ac 2n'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   9.0605(17)
_cell_length_b                   7.1533(15)
_cell_length_c                   11.213(2)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     726.7(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    1465
_cell_measurement_theta_min      2.89
_cell_measurement_theta_max      25.03

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.465
_exptl_crystal_F_000             700
_exptl_transmission_factor_min   0.864
_exptl_transmission_factor_max   0.864
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_exptl_absorpt_coefficient_mu    8.838
_shelx_estimated_absorpt_T_min   0.417
_shelx_estimated_absorpt_T_max   0.538
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   sadabs
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            7562
_diffrn_reflns_av_unetI/netI     0.0748
_diffrn_reflns_av_R_equivalents  0.1364
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_theta_min         3.378
_diffrn_reflns_theta_max         25.209
_diffrn_reflns_theta_full        25.209
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measured_fraction_theta_full 0.990
_diffrn_reflns_Laue_measured_fraction_max 0.990
_diffrn_reflns_Laue_measured_fraction_full 0.990
_diffrn_reflns_point_group_measured_fraction_max 0.990
_diffrn_reflns_point_group_measured_fraction_full 0.990
_reflns_number_total             707
_reflns_number_gt                523
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0135P)²+10.0072P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         707
_refine_ls_number_parameters     67
_refine_ls_number_restraints     12
_refine_ls_R_factor_all          0.0738
_refine_ls_R_factor_gt           0.0405
_refine_ls_wR_factor_ref         0.0757
_refine_ls_wR_factor_gt          0.0658
_refine_ls_goodness_of_fit_ref   1.016
_refine_ls_restrained_S_all      1.007
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
B1 B 0.5637(18) 0.7500 0.6278(15) 0.019(4) Uani 1 2 d S TU P . .
B2 B 0.9095(17) 0.2500 0.6184(16) 0.020(4) Uani 1 2 d S T P . .
K1 K 0.8004(2) 0.9963(3) 0.4020(2) 0.0232(6) Uani 1 1 d . . . . .
K2 K 0.4391(4) 0.7500 0.3696(3) 0.0547(13) Uani 1 2 d S T P . .
Nd1 Nd 0.87393(8) 0.7500 0.66804(7) 0.0127(2) Uani 1 2 d S T P . .
O1 O 0.4115(9) 0.7500 0.6144(8) 0.016(2) Uani 1 2 d S TU P . .
O2 O 0.6203(10) 0.7500 0.7409(8) 0.018(2) Uani 1 2 d S T P . .
O3 O 0.6593(9) 0.7500 0.5316(8) 0.018(2) Uani 1 2 d S T P . .
O4 O 0.8714(7) 0.4174(8) 0.6703(6) 0.0239(15) Uani 1 1 d . . . . .
O5 O 0.9910(9) 0.2500 0.5138(9) 0.016(2) Uani 1 2 d S T P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
B1 O2 1.368(18) . ?
B1 O3 1.383(18) . ?
B1 O1 1.387(18) . ?
B1 Nd1 2.847(16) . ?
B1 Nd1 2.863(17) 6_557 ?
B1 K2 3.108(17) . ?
B1 K2 3.5769(8) 5_666 ?
B1 K2 3.5769(8) 5_676 ?
B2 O4 1.375(10) . ?
B2 O4 1.375(10) 7_565 ?
B2 O5 1.386(19) . ?
B2 K2 3.132(18) 2_665 ?
B2 K2 3.162(16) 5_666 ?
B2 K1 3.172(13) 3_746 ?
B2 K1 3.172(13) 5_766 ?
B2 K1 3.188(15) 1_545 ?
B2 K1 3.188(15) 7_575 ?
K1 O3 2.617(7) . ?
K1 O1 2.648(6) 5_676 ?
K1 O2 2.660(7) 2_674 ?
K1 O5 2.751(7) 5_766 ?
K1 O5 2.801(7) 1_565 ?
K1 O4 3.081(7) 8_765 ?
K1 O4 3.133(7) 3_756 ?
K1 O4 3.138(7) 7_575 ?
K1 B2 3.172(13) 5_766 ?
K1 B2 3.188(15) 1_565 ?
K1 K1 3.523(5) 7_575 ?
K1 Nd1 3.528(2) . ?
K2 O3 2.698(9) . ?
K2 O1 2.757(10) . ?
K2 O4 3.062(7) 2_664 ?
K2 O4 3.062(7) 8_765 ?
K2 O4 3.091(7) 5_666 ?
K2 O4 3.091(7) 3_656 ?
K2 B2 3.132(18) 2_664 ?
K2 B2 3.162(16) 5_666 ?
K2 B1 3.5769(8) 5_666 ?
K2 B1 3.5769(8) 5_676 ?
Nd1 O4 2.380(6) . ?
Nd1 O4 2.380(6) 7_575 ?
Nd1 O5 2.378(9) 5_766 ?
Nd1 O2 2.439(10) . ?
Nd1 O2 2.455(10) 6_657 ?
Nd1 O1 2.463(9) 6_657 ?
Nd1 O3 2.474(9) . ?
Nd1 B1 2.863(17) 6_657 ?
Nd1 K1 3.528(2) 7_575 ?
Nd1 K1 3.552(2) 5_776 ?
O1 Nd1 2.463(9) 6_557 ?
O1 K1 2.648(6) 3_646 ?
O1 K1 2.648(6) 5_676 ?
O2 Nd1 2.455(9) 6_557 ?
O2 K1 2.660(7) 2_675 ?
O2 K1 2.660(7) 8_756 ?
O3 K1 2.617(7) 7_575 ?
O4 K2 3.062(7) 2_665 ?
O4 K1 3.081(7) 8_756 ?
O4 K2 3.091(7) 5_666 ?
O4 K1 3.133(7) 3_746 ?
O4 K1 3.137(7) 7_575 ?
O5 Nd1 2.378(9) 5_766 ?
O5 K1 2.751(7) 3_746 ?
O5 K1 2.751(7) 5_766 ?
O5 K1 2.801(7) 1_545 ?
O5 K1 2.801(7) 7_575 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 B1 O3 119.2(13) . . ?
O2 B1 O1 118.2(13) . . ?
O3 B1 O1 122.6(13) . . ?
O2 B1 Nd1 58.9(7) . . ?
O3 B1 Nd1 60.4(7) . . ?
O1 B1 Nd1 177.1(11) . . ?
O2 B1 Nd1 58.9(7) . 6_557 ?
O3 B1 Nd1 178.1(11) . 6_557 ?
O1 B1 Nd1 59.3(7) . 6_557 ?
Nd1 B1 Nd1 117.8(6) . 6_557 ?
O2 B1 K2 179.3(11) . . ?
O3 B1 K2 60.1(7) . . ?
O1 B1 K2 62.5(7) . . ?
Nd1 B1 K2 120.4(5) . . ?
Nd1 B1 K2 121.8(6) 6_557 . ?
O2 B1 K2 89.7(3) . 5_666 ?
O3 B1 K2 90.6(3) . 5_666 ?
O1 B1 K2 89.6(3) . 5_666 ?
Nd1 B1 K2 90.3(3) . 5_666 ?
Nd1 B1 K2 89.4(3) 6_557 5_666 ?
K2 B1 K2 90.3(3) . 5_666 ?
O2 B1 K2 89.7(3) . 5_676 ?
O3 B1 K2 90.6(3) . 5_676 ?
O1 B1 K2 89.6(3) . 5_676 ?
Nd1 B1 K2 90.3(3) . 5_676 ?
Nd1 B1 K2 89.4(3) 6_557 5_676 ?
K2 B1 K2 90.3(3) . 5_676 ?
K2 B1 K2 178.7(6) 5_666 5_676 ?
O4 B2 O4 121.1(13) . 7_565 ?
O4 B2 O5 119.4(7) . . ?
O4 B2 O5 119.4(7) 7_565 . ?
O4 B2 K2 74.3(8) . 2_665 ?
O4 B2 K2 74.3(8) 7_565 2_665 ?
O5 B2 K2 121.9(9) . 2_665 ?
O4 B2 K2 74.4(7) . 5_666 ?
O4 B2 K2 74.4(7) 7_565 5_666 ?
O5 B2 K2 124.6(10) . 5_666 ?
K2 B2 K2 113.5(5) 2_665 5_666 ?
O4 B2 K1 75.8(5) . 3_746 ?
O4 B2 K1 136.2(9) 7_565 3_746 ?
O5 B2 K1 59.9(5) . 3_746 ?
K2 B2 K1 72.7(3) 2_665 3_746 ?
K2 B2 K1 146.18(16) 5_666 3_746 ?
O4 B2 K1 136.2(9) . 5_766 ?
O4 B2 K1 75.8(5) 7_565 5_766 ?
O5 B2 K1 59.9(5) . 5_766 ?
K2 B2 K1 72.7(3) 2_665 5_766 ?
K2 B2 K1 146.18(16) 5_666 5_766 ?
K1 B2 K1 67.5(3) 3_746 5_766 ?
O4 B2 K1 137.7(10) . 1_545 ?
O4 B2 K1 75.4(6) 7_565 1_545 ?
O5 B2 K1 61.4(6) . 1_545 ?
K2 B2 K1 145.11(19) 2_665 1_545 ?
K2 B2 K1 73.9(3) 5_666 1_545 ?
K1 B2 K1 121.2(5) 3_746 1_545 ?
K1 B2 K1 83.4(3) 5_766 1_545 ?
O4 B2 K1 75.4(6) . 7_575 ?
O4 B2 K1 137.7(10) 7_565 7_575 ?
O5 B2 K1 61.4(6) . 7_575 ?
K2 B2 K1 145.11(19) 2_665 7_575 ?
K2 B2 K1 73.9(3) 5_666 7_575 ?
K1 B2 K1 83.4(3) 3_746 7_575 ?
K1 B2 K1 121.2(5) 5_766 7_575 ?
K1 B2 K1 69.4(4) 1_545 7_575 ?
O3 K1 O1 98.4(2) . 5_676 ?
O3 K1 O2 165.6(3) . 2_674 ?
O1 K1 O2 71.4(3) 5_676 2_674 ?
O3 K1 O5 73.4(2) . 5_766 ?
O1 K1 O5 163.9(3) 5_676 5_766 ?
O2 K1 O5 119.0(3) 2_674 5_766 ?
O3 K1 O5 119.2(3) . 1_565 ?
O1 K1 O5 91.94(19) 5_676 1_565 ?
O2 K1 O5 72.3(3) 2_674 1_565 ?
O5 K1 O5 80.66(6) 5_766 1_565 ?
O3 K1 O4 95.6(2) . 8_765 ?
O1 K1 O4 72.6(2) 5_676 8_765 ?
O2 K1 O4 71.9(2) 2_674 8_765 ?
O5 K1 O4 121.3(2) 5_766 8_765 ?
O5 K1 O4 143.9(2) 1_565 8_765 ?
O3 K1 O4 119.07(19) . 3_756 ?
O1 K1 O4 142.5(2) 5_676 3_756 ?
O2 K1 O4 72.0(2) 2_674 3_756 ?
O5 K1 O4 47.2(2) 5_766 3_756 ?
O5 K1 O4 69.4(2) 1_565 3_756 ?
O4 K1 O4 103.20(12) 8_765 3_756 ?
O3 K1 O4 72.6(2) . 7_575 ?
O1 K1 O4 94.6(2) 5_676 7_575 ?
O2 K1 O4 117.5(2) 2_674 7_575 ?
O5 K1 O4 69.9(2) 5_766 7_575 ?
O5 K1 O4 46.9(2) 1_565 7_575 ?
O4 K1 O4 161.49(11) 8_765 7_575 ?
O4 K1 O4 95.08(17) 3_756 7_575 ?
O3 K1 B2 94.1(3) . 5_766 ?
O1 K1 B2 167.5(3) 5_676 5_766 ?
O2 K1 B2 96.1(3) 2_674 5_766 ?
O5 K1 B2 25.8(4) 5_766 5_766 ?
O5 K1 B2 83.2(3) 1_565 5_766 ?
O4 K1 B2 104.8(3) 8_765 5_766 ?
O4 K1 B2 25.2(2) 3_756 5_766 ?
O4 K1 B2 90.5(3) 7_575 5_766 ?
O3 K1 B2 96.4(3) . 1_565 ?
O1 K1 B2 83.5(3) 5_676 1_565 ?
O2 K1 B2 92.6(3) 2_674 1_565 ?
O5 K1 B2 83.7(3) 5_766 1_565 ?
O5 K1 B2 25.7(3) 1_565 1_565 ?
O4 K1 B2 154.6(2) 8_765 1_565 ?
O4 K1 B2 90.3(3) 3_756 1_565 ?
O4 K1 B2 25.1(2) 7_575 1_565 ?
B2 K1 B2 96.5(3) 5_766 1_565 ?
O3 K1 K1 47.70(13) . 7_575 ?
O1 K1 K1 133.26(13) 5_676 7_575 ?
O2 K1 K1 133.03(14) 2_674 7_575 ?
O5 K1 K1 50.19(12) 5_766 7_575 ?
O5 K1 K1 130.38(12) 1_565 7_575 ?
O4 K1 K1 79.45(12) 8_765 7_575 ?
O4 K1 K1 79.62(12) 3_756 7_575 ?
O4 K1 K1 101.35(12) 7_575 7_575 ?
B2 K1 K1 56.27(16) 5_766 7_575 ?
B2 K1 K1 124.71(19) 1_565 7_575 ?
O3 K1 Nd1 44.48(19) . . ?
O1 K1 Nd1 122.5(2) 5_676 . ?
O2 K1 Nd1 149.8(2) 2_674 . ?
O5 K1 Nd1 42.3(2) 5_766 . ?
O5 K1 Nd1 80.13(17) 1_565 . ?
O4 K1 Nd1 135.81(14) 8_765 . ?
O4 K1 Nd1 87.10(13) 3_756 . ?
O4 K1 Nd1 41.31(11) 7_575 . ?
B2 K1 Nd1 68.1(3) 5_766 . ?
B2 K1 Nd1 65.29(19) 1_565 . ?
K1 K1 Nd1 60.04(4) 7_575 . ?
O3 K2 O1 52.9(2) . . ?
O3 K2 O4 94.4(2) . 2_664 ?
O1 K2 O4 141.1(2) . 2_664 ?
O3 K2 O4 94.4(2) . 8_765 ?
O1 K2 O4 141.1(2) . 8_765 ?
O4 K2 O4 46.0(2) 2_664 8_765 ?
O3 K2 O4 140.4(2) . 5_666 ?
O1 K2 O4 93.5(2) . 5_666 ?
O4 K2 O4 104.68(16) 2_664 5_666 ?
O4 K2 O4 123.80(16) 8_765 5_666 ?
O3 K2 O4 140.4(2) . 3_656 ?
O1 K2 O4 93.5(2) . 3_656 ?
O4 K2 O4 123.80(16) 2_664 3_656 ?
O4 K2 O4 104.68(16) 8_765 3_656 ?
O4 K2 O4 45.6(2) 5_666 3_656 ?
O3 K2 B1 26.4(4) . . ?
O1 K2 B1 26.5(3) . . ?
O4 K2 B1 118.5(3) 2_664 . ?
O4 K2 B1 118.5(3) 8_765 . ?
O4 K2 B1 117.7(3) 5_666 . ?
O4 K2 B1 117.7(3) 3_656 . ?
O3 K2 B2 106.4(4) . 2_664 ?
O1 K2 B2 159.3(4) . 2_664 ?
O4 K2 B2 25.62(17) 2_664 2_664 ?
O4 K2 B2 25.62(17) 8_765 2_664 ?
O4 K2 B2 105.6(3) 5_666 2_664 ?
O4 K2 B2 105.6(3) 3_656 2_664 ?
B1 K2 B2 132.7(4) . 2_664 ?
O3 K2 B2 135.2(4) . 5_666 ?
O1 K2 B2 82.3(4) . 5_666 ?
O4 K2 B2 126.2(3) 2_664 5_666 ?
O4 K2 B2 126.2(3) 8_765 5_666 ?
O4 K2 B2 25.37(18) 5_666 5_666 ?
O4 K2 B2 25.37(18) 3_656 5_666 ?
B1 K2 B2 108.9(5) . 5_666 ?
B2 K2 B2 118.4(3) 2_664 5_666 ?
O3 K2 B1 90.0(3) . 5_666 ?
O1 K2 B1 89.5(3) . 5_666 ?
O4 K2 B1 67.6(3) 2_664 5_666 ?
O4 K2 B1 113.6(3) 8_765 5_666 ?
O4 K2 B1 66.9(3) 5_666 5_666 ?
O4 K2 B1 112.5(3) 3_656 5_666 ?
B1 K2 B1 89.7(3) . 5_666 ?
B2 K2 B1 90.6(3) 2_664 5_666 ?
B2 K2 B1 89.6(3) 5_666 5_666 ?
O3 K2 B1 90.0(3) . 5_676 ?
O1 K2 B1 89.5(3) . 5_676 ?
O4 K2 B1 113.6(3) 2_664 5_676 ?
O4 K2 B1 67.6(3) 8_765 5_676 ?
O4 K2 B1 112.5(3) 5_666 5_676 ?
O4 K2 B1 66.9(3) 3_656 5_676 ?
B1 K2 B1 89.7(3) . 5_676 ?
B2 K2 B1 90.6(3) 2_664 5_676 ?
B2 K2 B1 89.6(3) 5_666 5_676 ?
B1 K2 B1 178.7(6) 5_666 5_676 ?
O3 K2 K1 44.49(14) . . ?
O1 K2 K1 89.01(18) . . ?
O4 K2 K1 76.37(14) 2_664 . ?
O4 K2 K1 52.80(13) 8_765 . ?
O4 K2 K1 174.13(14) 5_666 . ?
O4 K2 K1 129.00(12) 3_656 . ?
B1 K2 K1 65.9(3) . . ?
B2 K2 K1 72.8(3) 2_664 . ?
B2 K2 K1 150.63(11) 5_666 . ?
B1 K2 K1 118.5(3) 5_666 . ?
B1 K2 K1 62.2(3) 5_676 . ?
O4 Nd1 O4 178.4(3) . 7_575 ?
O4 Nd1 O5 90.79(16) . 5_766 ?
O4 Nd1 O5 90.79(16) 7_575 5_766 ?
O4 Nd1 O2 89.29(16) . . ?
O4 Nd1 O2 89.29(16) 7_575 . ?
O5 Nd1 O2 140.6(3) 5_766 . ?
O4 Nd1 O2 90.24(16) . 6_657 ?
O4 Nd1 O2 90.24(16) 7_575 6_657 ?
O5 Nd1 O2 83.6(3) 5_766 6_657 ?
O2 Nd1 O2 135.85(4) . 6_657 ?
O4 Nd1 O1 89.48(16) . 6_657 ?
O4 Nd1 O1 89.48(16) 7_575 6_657 ?
O5 Nd1 O1 141.1(3) 5_766 6_657 ?
O2 Nd1 O1 78.4(3) . 6_657 ?
O2 Nd1 O1 57.5(3) 6_657 6_657 ?
O4 Nd1 O3 89.94(16) . . ?
O4 Nd1 O3 89.94(16) 7_575 . ?
O5 Nd1 O3 82.8(3) 5_766 . ?
O2 Nd1 O3 57.8(3) . . ?
O2 Nd1 O3 166.4(3) 6_657 . ?
O1 Nd1 O3 136.1(3) 6_657 . ?
O4 Nd1 B1 89.56(16) . . ?
O4 Nd1 B1 89.56(16) 7_575 . ?
O5 Nd1 B1 111.9(4) 5_766 . ?
O2 Nd1 B1 28.7(4) . . ?
O2 Nd1 B1 164.5(4) 6_657 . ?
O1 Nd1 B1 107.1(4) 6_657 . ?
O3 Nd1 B1 29.1(4) . . ?
O4 Nd1 B1 89.85(16) . 6_657 ?
O4 Nd1 B1 89.85(16) 7_575 6_657 ?
O5 Nd1 B1 112.1(4) 5_766 6_657 ?
O2 Nd1 B1 107.3(4) . 6_657 ?
O2 Nd1 B1 28.5(4) 6_657 6_657 ?
O1 Nd1 B1 29.0(4) 6_657 6_657 ?
O3 Nd1 B1 165.1(4) . 6_657 ?
B1 Nd1 B1 136.0(3) . 6_657 ?
O4 Nd1 K1 60.51(16) . 7_575 ?
O4 Nd1 K1 120.42(17) 7_575 7_575 ?
O5 Nd1 K1 51.12(16) 5_766 7_575 ?
O2 Nd1 K1 96.04(18) . 7_575 ?
O2 Nd1 K1 121.57(17) 6_657 7_575 ?
O1 Nd1 K1 149.72(5) 6_657 7_575 ?
O3 Nd1 K1 47.84(15) . 7_575 ?
B1 Nd1 K1 71.3(3) . 7_575 ?
B1 Nd1 K1 142.1(2) 6_657 7_575 ?
O4 Nd1 K1 120.42(17) . . ?
O4 Nd1 K1 60.51(16) 7_575 . ?
O5 Nd1 K1 51.12(16) 5_766 . ?
O2 Nd1 K1 96.04(18) . . ?
O2 Nd1 K1 121.57(17) 6_657 . ?
O1 Nd1 K1 149.72(5) 6_657 . ?
O3 Nd1 K1 47.84(15) . . ?
B1 Nd1 K1 71.3(3) . . ?
B1 Nd1 K1 142.1(2) 6_657 . ?
K1 Nd1 K1 59.91(8) 7_575 . ?
O4 Nd1 K1 121.40(16) . 5_776 ?
O4 Nd1 K1 59.95(16) 7_575 5_776 ?
O5 Nd1 K1 51.89(16) 5_766 5_776 ?
O2 Nd1 K1 148.96(5) . 5_776 ?
O2 Nd1 K1 48.43(15) 6_657 5_776 ?
O1 Nd1 K1 95.98(17) 6_657 5_776 ?
O3 Nd1 K1 121.08(16) . 5_776 ?
B1 Nd1 K1 141.74(19) . 5_776 ?
B1 Nd1 K1 71.2(3) 6_657 5_776 ?
K1 Nd1 K1 103.01(4) 7_575 5_776 ?
K1 Nd1 K1 73.43(6) . 5_776 ?
B1 O1 Nd1 91.7(8) . 6_557 ?
B1 O1 K1 136.73(13) . 3_646 ?
Nd1 O1 K1 88.2(2) 6_557 3_646 ?
B1 O1 K1 136.73(13) . 5_676 ?
Nd1 O1 K1 88.2(2) 6_557 5_676 ?
K1 O1 K1 86.5(3) 3_646 5_676 ?
B1 O1 K2 91.0(8) . . ?
Nd1 O1 K2 177.3(4) 6_557 . ?
K1 O1 K2 89.8(2) 3_646 . ?
K1 O1 K2 89.8(2) 5_676 . ?
B1 O2 Nd1 92.5(8) . . ?
B1 O2 Nd1 92.6(8) . 6_557 ?
Nd1 O2 Nd1 175.0(4) . 6_557 ?
B1 O2 K1 136.97(14) . 2_675 ?
Nd1 O2 K1 88.5(3) . 2_675 ?
Nd1 O2 K1 87.9(2) 6_557 2_675 ?
B1 O2 K1 136.97(14) . 8_756 ?
Nd1 O2 K1 88.5(3) . 8_756 ?
Nd1 O2 K1 87.9(2) 6_557 8_756 ?
K1 O2 K1 86.1(3) 2_675 8_756 ?
B1 O3 Nd1 90.6(8) . . ?
B1 O3 K1 137.63(14) . 7_575 ?
Nd1 O3 K1 87.7(2) . 7_575 ?
B1 O3 K1 137.63(14) . . ?
Nd1 O3 K1 87.7(2) . . ?
K1 O3 K1 84.6(3) 7_575 . ?
B1 O3 K2 93.6(8) . . ?
Nd1 O3 K2 175.8(4) . . ?
K1 O3 K2 89.3(2) 7_575 . ?
K1 O3 K2 89.3(2) . . ?
B2 O4 Nd1 149.8(7) . . ?
B2 O4 K2 80.1(8) . 2_665 ?
Nd1 O4 K2 113.2(2) . 2_665 ?
B2 O4 K1 130.0(7) . 8_756 ?
Nd1 O4 K1 80.24(18) . 8_756 ?
K2 O4 K1 74.88(17) 2_665 8_756 ?
B2 O4 K2 80.2(7) . 5_666 ?
Nd1 O4 K2 113.2(2) . 5_666 ?
K2 O4 K2 117.7(2) 2_665 5_666 ?
K1 O4 K2 74.50(16) 8_756 5_666 ?
B2 O4 K1 79.0(7) . 3_746 ?
Nd1 O4 K1 78.94(17) . 3_746 ?
K2 O4 K1 74.17(17) 2_665 3_746 ?
K1 O4 K1 131.6(2) 8_756 3_746 ?
K2 O4 K1 153.7(2) 5_666 3_746 ?
B2 O4 K1 79.5(8) . 7_575 ?
Nd1 O4 K1 78.17(18) . 7_575 ?
K2 O4 K1 153.1(2) 2_665 7_575 ?
K1 O4 K1 132.0(2) 8_756 7_575 ?
K2 O4 K1 75.57(17) 5_666 7_575 ?
K1 O4 K1 84.92(17) 3_746 7_575 ?
B2 O5 Nd1 178.8(9) . 5_766 ?
B2 O5 K1 94.3(6) . 3_746 ?
Nd1 O5 K1 86.6(2) 5_766 3_746 ?
B2 O5 K1 94.3(6) . 5_766 ?
Nd1 O5 K1 86.6(2) 5_766 5_766 ?
K1 O5 K1 79.6(2) 3_746 5_766 ?
B2 O5 K1 92.9(6) . 1_545 ?
Nd1 O5 K1 86.2(3) 5_766 1_545 ?
K1 O5 K1 172.8(4) 3_746 1_545 ?
K1 O5 K1 99.34(7) 5_766 1_545 ?
B2 O5 K1 92.9(6) . 7_575 ?
Nd1 O5 K1 86.2(3) 5_766 7_575 ?
K1 O5 K1 99.34(7) 3_746 7_575 ?
K1 O5 K1 172.8(4) 5_766 7_575 ?
K1 O5 K1 80.8(2) 1_545 7_575 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 B1 O1 Nd1 0.000(3) . . . 6_557 ?
O3 B1 O1 Nd1 180.000(3) . . . 6_557 ?
K2 B1 O1 Nd1 180.000(1) . . . 6_557 ?
K2 B1 O1 Nd1 89.5(3) 5_666 . . 6_557 ?
K2 B1 O1 Nd1 -89.5(3) 5_676 . . 6_557 ?
O2 B1 O1 K1 -89.2(10) . . . 3_646 ?
O3 B1 O1 K1 90.8(10) . . . 3_646 ?
Nd1 B1 O1 K1 -89.2(10) 6_557 . . 3_646 ?
K2 B1 O1 K1 90.8(10) . . . 3_646 ?
K2 B1 O1 K1 0.3(12) 5_666 . . 3_646 ?
K2 B1 O1 K1 -178.7(8) 5_676 . . 3_646 ?
O2 B1 O1 K1 89.2(10) . . . 5_676 ?
O3 B1 O1 K1 -90.8(10) . . . 5_676 ?
Nd1 B1 O1 K1 89.2(10) 6_557 . . 5_676 ?
K2 B1 O1 K1 -90.8(10) . . . 5_676 ?
K2 B1 O1 K1 178.7(8) 5_666 . . 5_676 ?
K2 B1 O1 K1 -0.3(12) 5_676 . . 5_676 ?
O2 B1 O1 K2 180.000(3) . . . . ?
O3 B1 O1 K2 0.000(2) . . . . ?
Nd1 B1 O1 K2 180.000(2) 6_557 . . . ?
K2 B1 O1 K2 -90.5(3) 5_666 . . . ?
K2 B1 O1 K2 90.5(3) 5_676 . . . ?
O3 B1 O2 Nd1 0.000(2) . . . . ?
O1 B1 O2 Nd1 180.000(3) . . . . ?
Nd1 B1 O2 Nd1 180.000(2) 6_557 . . . ?
K2 B1 O2 Nd1 90.6(3) 5_666 . . . ?
K2 B1 O2 Nd1 -90.6(3) 5_676 . . . ?
O3 B1 O2 Nd1 180.000(2) . . . 6_557 ?
O1 B1 O2 Nd1 0.000(3) . . . 6_557 ?
Nd1 B1 O2 Nd1 180.000(1) . . . 6_557 ?
K2 B1 O2 Nd1 -89.4(3) 5_666 . . 6_557 ?
K2 B1 O2 Nd1 89.4(3) 5_676 . . 6_557 ?
O3 B1 O2 K1 90.4(11) . . . 2_675 ?
O1 B1 O2 K1 -89.6(11) . . . 2_675 ?
Nd1 B1 O2 K1 90.4(11) . . . 2_675 ?
Nd1 B1 O2 K1 -89.6(11) 6_557 . . 2_675 ?
K2 B1 O2 K1 -179.1(9) 5_666 . . 2_675 ?
K2 B1 O2 K1 -0.2(13) 5_676 . . 2_675 ?
O3 B1 O2 K1 -90.4(11) . . . 8_756 ?
O1 B1 O2 K1 89.6(11) . . . 8_756 ?
Nd1 B1 O2 K1 -90.4(11) . . . 8_756 ?
Nd1 B1 O2 K1 89.6(11) 6_557 . . 8_756 ?
K2 B1 O2 K1 0.2(13) 5_666 . . 8_756 ?
K2 B1 O2 K1 179.1(9) 5_676 . . 8_756 ?
O2 B1 O3 Nd1 0.000(3) . . . . ?
O1 B1 O3 Nd1 180.000(3) . . . . ?
K2 B1 O3 Nd1 180.000(1) . . . . ?
K2 B1 O3 Nd1 -90.0(3) 5_666 . . . ?
K2 B1 O3 Nd1 90.0(3) 5_676 . . . ?
O2 B1 O3 K1 87.2(10) . . . 7_575 ?
O1 B1 O3 K1 -92.8(10) . . . 7_575 ?
Nd1 B1 O3 K1 87.2(10) . . . 7_575 ?
K2 B1 O3 K1 -92.8(10) . . . 7_575 ?
K2 B1 O3 K1 -2.8(12) 5_666 . . 7_575 ?
K2 B1 O3 K1 177.2(8) 5_676 . . 7_575 ?
O2 B1 O3 K1 -87.2(10) . . . . ?
O1 B1 O3 K1 92.8(10) . . . . ?
Nd1 B1 O3 K1 -87.2(10) . . . . ?
K2 B1 O3 K1 92.8(10) . . . . ?
K2 B1 O3 K1 -177.2(8) 5_666 . . . ?
K2 B1 O3 K1 2.8(12) 5_676 . . . ?
O2 B1 O3 K2 180.000(3) . . . . ?
O1 B1 O3 K2 0.000(3) . . . . ?
Nd1 B1 O3 K2 180.000(1) . . . . ?
K2 B1 O3 K2 90.0(3) 5_666 . . . ?
K2 B1 O3 K2 -90.0(3) 5_676 . . . ?
O4 B2 O4 Nd1 179.7(3) 7_565 . . . ?
O5 B2 O4 Nd1 1(3) . . . . ?
K2 B2 O4 Nd1 119.5(14) 2_665 . . . ?
K2 B2 O4 Nd1 -119.9(14) 5_666 . . . ?
K1 B2 O4 Nd1 43.8(15) 3_746 . . . ?
K1 B2 O4 Nd1 77(2) 5_766 . . . ?
K1 B2 O4 Nd1 -77.3(19) 1_545 . . . ?
K1 B2 O4 Nd1 -43.0(15) 7_575 . . . ?
O4 B2 O4 K2 60.2(13) 7_565 . . 2_665 ?
O5 B2 O4 K2 -118.1(13) . . . 2_665 ?
K2 B2 O4 K2 120.6(2) 5_666 . . 2_665 ?
K1 B2 O4 K2 -75.64(19) 3_746 . . 2_665 ?
K1 B2 O4 K2 -42.3(11) 5_766 . . 2_665 ?
K1 B2 O4 K2 163.3(12) 1_545 . . 2_665 ?
K1 B2 O4 K2 -162.4(3) 7_575 . . 2_665 ?
O4 B2 O4 K1 0(2) 7_565 . . 8_756 ?
O5 B2 O4 K1 -178.6(7) . . . 8_756 ?
K2 B2 O4 K1 -60.5(7) 2_665 . . 8_756 ?
K2 B2 O4 K1 60.1(8) 5_666 . . 8_756 ?
K1 B2 O4 K1 -136.1(7) 3_746 . . 8_756 ?
K1 B2 O4 K1 -102.8(11) 5_766 . . 8_756 ?
K1 B2 O4 K1 102.8(12) 1_545 . . 8_756 ?
K1 B2 O4 K1 137.1(7) 7_575 . . 8_756 ?
O4 B2 O4 K2 -60.4(13) 7_565 . . 5_666 ?
O5 B2 O4 K2 121.3(13) . . . 5_666 ?
K2 B2 O4 K2 -120.6(2) 2_665 . . 5_666 ?
K1 B2 O4 K2 163.8(3) 3_746 . . 5_666 ?
K1 B2 O4 K2 -162.9(12) 5_766 . . 5_666 ?
K1 B2 O4 K2 42.7(10) 1_545 . . 5_666 ?
K1 B2 O4 K2 76.99(19) 7_575 . . 5_666 ?
O4 B2 O4 K1 135.8(14) 7_565 . . 3_746 ?
O5 B2 O4 K1 -42.5(12) . . . 3_746 ?
K2 B2 O4 K1 75.64(19) 2_665 . . 3_746 ?
K2 B2 O4 K1 -163.8(3) 5_666 . . 3_746 ?
K1 B2 O4 K1 33.4(10) 5_766 . . 3_746 ?
K1 B2 O4 K1 -121.1(11) 1_545 . . 3_746 ?
K1 B2 O4 K1 -86.8(2) 7_575 . . 3_746 ?
O4 B2 O4 K1 -137.4(14) 7_565 . . 7_575 ?
O5 B2 O4 K1 44.3(12) . . . 7_575 ?
K2 B2 O4 K1 162.4(3) 2_665 . . 7_575 ?
K2 B2 O4 K1 -76.99(19) 5_666 . . 7_575 ?
K1 B2 O4 K1 86.8(2) 3_746 . . 7_575 ?
K1 B2 O4 K1 120.2(12) 5_766 . . 7_575 ?
K1 B2 O4 K1 -34.3(10) 1_545 . . 7_575 ?
O4 B2 O5 K1 49.2(13) . . . 3_746 ?
O4 B2 O5 K1 -129.1(12) 7_565 . . 3_746 ?
K2 B2 O5 K1 -39.95(14) 2_665 . . 3_746 ?
K2 B2 O5 K1 140.05(14) 5_666 . . 3_746 ?
K1 B2 O5 K1 -79.9(3) 5_766 . . 3_746 ?
K1 B2 O5 K1 -179.5(3) 1_545 . . 3_746 ?
K1 B2 O5 K1 99.60(6) 7_575 . . 3_746 ?
O4 B2 O5 K1 129.1(12) . . . 5_766 ?
O4 B2 O5 K1 -49.2(13) 7_565 . . 5_766 ?
K2 B2 O5 K1 39.95(14) 2_665 . . 5_766 ?
K2 B2 O5 K1 -140.05(14) 5_666 . . 5_766 ?
K1 B2 O5 K1 79.9(3) 3_746 . . 5_766 ?
K1 B2 O5 K1 -99.60(6) 1_545 . . 5_766 ?
K1 B2 O5 K1 179.5(3) 7_575 . . 5_766 ?
O4 B2 O5 K1 -131.3(12) . . . 1_545 ?
O4 B2 O5 K1 50.4(13) 7_565 . . 1_545 ?
K2 B2 O5 K1 139.55(13) 2_665 . . 1_545 ?
K2 B2 O5 K1 -40.45(13) 5_666 . . 1_545 ?
K1 B2 O5 K1 179.5(3) 3_746 . . 1_545 ?
K1 B2 O5 K1 99.60(6) 5_766 . . 1_545 ?
K1 B2 O5 K1 -80.9(3) 7_575 . . 1_545 ?
O4 B2 O5 K1 -50.4(13) . . . 7_575 ?
O4 B2 O5 K1 131.3(12) 7_565 . . 7_575 ?
K2 B2 O5 K1 -139.55(13) 2_665 . . 7_575 ?
K2 B2 O5 K1 40.45(13) 5_666 . . 7_575 ?
K1 B2 O5 K1 -99.60(6) 3_746 . . 7_575 ?
K1 B2 O5 K1 -179.5(3) 5_766 . . 7_575 ?
K1 B2 O5 K1 80.9(3) 1_545 . . 7_575 ?

_refine_diff_density_max         1.159
_refine_diff_density_min         -1.351
_refine_diff_density_rms         0.288



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_a_CCDC2
_database_code_depnum_ccdc_archive 'CCDC 2169923'
loop_
_audit_author_name
_audit_author_address
'Jingcheng Feng'
;Technical Institution of Physics and Chemistry, Chinese Academy of Sciences
China
;
_audit_update_record             
;
2022-05-02 deposited with the CCDC.	2022-07-10 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'B4 Gd2 K6 O12'
_chemical_formula_weight         784.34

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_H-M_alt        'P n m a'
_space_group_name_Hall           '-P 2ac 2n'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'

_cell_length_a                   8.9588(13)
_cell_length_b                   7.0621(10)
_cell_length_c                   11.1427(14)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     704.98(17)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    2005
_cell_measurement_theta_min      2.92
_cell_measurement_theta_max      30.48

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.695
_exptl_crystal_F_000             716
_exptl_transmission_factor_min   0.864
_exptl_transmission_factor_max   0.864
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_exptl_absorpt_coefficient_mu    11.154
_shelx_estimated_absorpt_T_min   0.348
_shelx_estimated_absorpt_T_max   0.469
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   sadabs
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ccd
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            5042
_diffrn_reflns_av_unetI/netI     0.0785
_diffrn_reflns_av_R_equivalents  0.0837
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_theta_min         2.917
_diffrn_reflns_theta_max         30.511
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.984
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.984
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.984
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             1139
_reflns_number_gt                870
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0154P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_extinction_coef       0.0201(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1139
_refine_ls_number_parameters     68
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0571
_refine_ls_R_factor_gt           0.0368
_refine_ls_wR_factor_ref         0.0694
_refine_ls_wR_factor_gt          0.0617
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_restrained_S_all      1.043
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
B1 B 0.0643(11) 0.2500 0.6272(8) 0.0096(19) Uani 1 2 d S T P . .
B2 B 0.5878(10) 0.2500 0.3840(8) 0.013(2) Uani 1 2 d S T P . .
Gd1 Gd 0.37457(4) 0.2500 0.66882(3) 0.00751(16) Uani 1 2 d S T P . .
K1 K -0.0609(3) 0.2500 0.37007(18) 0.0449(7) Uani 1 2 d S T P . .
K2 K 0.30038(15) 0.49461(19) 0.40220(10) 0.0175(3) Uani 1 1 d . . . . .
O1 O -0.0882(6) 0.2500 0.6162(5) 0.0134(13) Uani 1 2 d S T P . .
O2 O 0.1225(5) 0.2500 0.7434(4) 0.0127(13) Uani 1 2 d S T P . .
O3 O 0.1631(6) 0.2500 0.5347(5) 0.0161(13) Uani 1 2 d S T P . .
O4 O 0.5085(6) 0.2500 0.4907(5) 0.0112(12) Uani 1 2 d S T P . .
O5 O 0.6267(4) 0.0798(6) 0.3307(3) 0.0168(10) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
B1 O3 1.358(10) . ?
B1 O1 1.373(10) . ?
B1 O2 1.396(10) . ?
B1 Gd1 2.818(10) . ?
B1 Gd1 2.838(9) 6_557 ?
B1 K1 3.077(9) . ?
B1 K1 3.5313(5) 5_566 ?
B1 K1 3.5313(5) 5_556 ?
B2 O5 1.385(6) . ?
B2 O5 1.385(6) 7_565 ?
B2 O4 1.385(10) . ?
B2 K2 3.107(8) 7_565 ?
B2 K2 3.107(8) . ?
B2 K1 3.128(9) 6_656 ?
B2 K2 3.152(8) 5_666 ?
B2 K2 3.152(8) 3_646 ?
B2 K1 3.152(9) 1_655 ?
Gd1 O4 2.319(5) . ?
Gd1 O5 2.329(4) 3_656 ?
Gd1 O5 2.329(4) 5_656 ?
Gd1 O2 2.406(5) . ?
Gd1 O3 2.413(5) . ?
Gd1 O1 2.419(5) 6_657 ?
Gd1 O2 2.427(5) 6_657 ?
Gd1 B1 2.838(9) 6_657 ?
Gd1 K2 3.5002(12) . ?
Gd1 K2 3.5002(12) 7_565 ?
Gd1 K2 3.5156(14) 5_666 ?
K1 O3 2.718(6) . ?
K1 O1 2.753(6) . ?
K1 O5 3.045(4) 6_556 ?
K1 O5 3.045(4) 4_455 ?
K1 O5 3.077(4) 1_455 ?
K1 O5 3.077(4) 7_465 ?
K1 B2 3.128(9) 6_556 ?
K1 B2 3.152(9) 1_455 ?
K1 B1 3.5313(5) 5_556 ?
K1 B1 3.5313(5) 5_566 ?
K1 K2 3.686(2) . ?
K2 O3 2.584(4) . ?
K2 O2 2.619(4) 2_564 ?
K2 O1 2.628(4) 5_566 ?
K2 O4 2.726(4) . ?
K2 O4 2.759(4) 5_666 ?
K2 O5 3.071(4) 4_455 ?
K2 O5 3.076(4) 7_565 ?
K2 O5 3.106(4) 3_656 ?
K2 B2 3.152(8) 5_666 ?
K2 K2 3.455(3) 7_565 ?
O1 Gd1 2.419(5) 6_557 ?
O1 K2 2.628(4) 3_546 ?
O1 K2 2.628(4) 5_566 ?
O2 Gd1 2.427(5) 6_557 ?
O2 K2 2.619(4) 2_565 ?
O2 K2 2.619(4) 8_656 ?
O3 K2 2.584(4) 7_565 ?
O4 K2 2.726(4) 7_565 ?
O4 K2 2.759(4) 5_666 ?
O4 K2 2.759(4) 3_646 ?
O5 Gd1 2.329(4) 5_656 ?
O5 K1 3.045(4) 6_656 ?
O5 K2 3.071(4) 4 ?
O5 K2 3.076(4) 7_565 ?
O5 K1 3.077(4) 1_655 ?
O5 K2 3.106(4) 3_646 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 B1 O1 125.5(8) . . ?
O3 B1 O2 117.5(7) . . ?
O1 B1 O2 117.0(7) . . ?
O3 B1 Gd1 58.8(4) . . ?
O1 B1 Gd1 175.7(6) . . ?
O2 B1 Gd1 58.6(4) . . ?
O3 B1 Gd1 176.2(6) . 6_557 ?
O1 B1 Gd1 58.3(4) . 6_557 ?
O2 B1 Gd1 58.7(4) . 6_557 ?
Gd1 B1 Gd1 117.3(3) . 6_557 ?
O3 B1 K1 62.0(4) . . ?
O1 B1 K1 63.5(4) . . ?
O2 B1 K1 179.5(6) . . ?
Gd1 B1 K1 120.9(3) . . ?
Gd1 B1 K1 121.8(3) 6_557 . ?
O3 B1 K1 90.71(15) . 5_566 ?
O1 B1 K1 89.54(16) . 5_566 ?
O2 B1 K1 89.73(16) . 5_566 ?
Gd1 B1 K1 90.42(16) . 5_566 ?
Gd1 B1 K1 89.30(15) 6_557 5_566 ?
K1 B1 K1 90.27(16) . 5_566 ?
O3 B1 K1 90.71(15) . 5_556 ?
O1 B1 K1 89.54(16) . 5_556 ?
O2 B1 K1 89.73(16) . 5_556 ?
Gd1 B1 K1 90.42(16) . 5_556 ?
Gd1 B1 K1 89.30(15) 6_557 5_556 ?
K1 B1 K1 90.27(16) . 5_556 ?
K1 B1 K1 178.6(3) 5_566 5_556 ?
O5 B2 O5 120.4(7) . 7_565 ?
O5 B2 O4 119.8(4) . . ?
O5 B2 O4 119.8(4) 7_565 . ?
O5 B2 K2 75.8(3) . 7_565 ?
O5 B2 K2 136.0(5) 7_565 7_565 ?
O4 B2 K2 61.2(3) . 7_565 ?
O5 B2 K2 136.0(5) . . ?
O5 B2 K2 75.8(3) 7_565 . ?
O4 B2 K2 61.2(3) . . ?
K2 B2 K2 67.55(19) 7_565 . ?
O5 B2 K1 73.7(4) . 6_656 ?
O5 B2 K1 73.7(4) 7_565 6_656 ?
O4 B2 K1 123.9(5) . 6_656 ?
K2 B2 K1 72.93(19) 7_565 6_656 ?
K2 B2 K1 72.93(19) . 6_656 ?
O5 B2 K2 137.8(5) . 5_666 ?
O5 B2 K2 75.4(3) 7_565 5_666 ?
O4 B2 K2 60.9(3) . 5_666 ?
K2 B2 K2 122.2(3) 7_565 5_666 ?
K2 B2 K2 84.02(15) . 5_666 ?
K1 B2 K2 145.02(10) 6_656 5_666 ?
O5 B2 K2 75.4(3) . 3_646 ?
O5 B2 K2 137.8(5) 7_565 3_646 ?
O4 B2 K2 60.9(3) . 3_646 ?
K2 B2 K2 84.02(15) 7_565 3_646 ?
K2 B2 K2 122.2(3) . 3_646 ?
K1 B2 K2 145.02(10) 6_656 3_646 ?
K2 B2 K2 69.82(19) 5_666 3_646 ?
O5 B2 K1 74.2(4) . 1_655 ?
O5 B2 K1 74.2(4) 7_565 1_655 ?
O4 B2 K1 123.7(5) . 1_655 ?
K2 B2 K1 146.19(10) 7_565 1_655 ?
K2 B2 K1 146.19(10) . 1_655 ?
K1 B2 K1 112.4(3) 6_656 1_655 ?
K2 B2 K1 73.72(19) 5_666 1_655 ?
K2 B2 K1 73.72(19) 3_646 1_655 ?
O4 Gd1 O5 90.26(9) . 3_656 ?
O4 Gd1 O5 90.26(9) . 5_656 ?
O5 Gd1 O5 179.37(19) 3_656 5_656 ?
O4 Gd1 O2 141.36(17) . . ?
O5 Gd1 O2 89.69(9) 3_656 . ?
O5 Gd1 O2 89.69(9) 5_656 . ?
O4 Gd1 O3 82.88(17) . . ?
O5 Gd1 O3 89.86(10) 3_656 . ?
O5 Gd1 O3 89.86(10) 5_656 . ?
O2 Gd1 O3 58.48(15) . . ?
O4 Gd1 O1 140.94(17) . 6_657 ?
O5 Gd1 O1 89.91(9) 3_656 6_657 ?
O5 Gd1 O1 89.91(9) 5_656 6_657 ?
O2 Gd1 O1 77.70(17) . 6_657 ?
O3 Gd1 O1 136.18(17) . 6_657 ?
O4 Gd1 O2 82.61(17) . 6_657 ?
O5 Gd1 O2 90.21(10) 3_656 6_657 ?
O5 Gd1 O2 90.21(10) 5_656 6_657 ?
O2 Gd1 O2 136.027(17) . 6_657 ?
O3 Gd1 O2 165.49(15) . 6_657 ?
O1 Gd1 O2 58.33(16) 6_657 6_657 ?
O4 Gd1 B1 111.7(2) . . ?
O5 Gd1 B1 89.74(10) 3_656 . ?
O5 Gd1 B1 89.74(10) 5_656 . ?
O2 Gd1 B1 29.7(2) . . ?
O3 Gd1 B1 28.8(2) . . ?
O1 Gd1 B1 107.4(2) 6_657 . ?
O2 Gd1 B1 165.7(2) 6_657 . ?
O4 Gd1 B1 112.1(2) . 6_657 ?
O5 Gd1 B1 90.07(9) 3_656 6_657 ?
O5 Gd1 B1 90.07(9) 5_656 6_657 ?
O2 Gd1 B1 106.6(2) . 6_657 ?
O3 Gd1 B1 165.1(2) . 6_657 ?
O1 Gd1 B1 28.9(2) 6_657 6_657 ?
O2 Gd1 B1 29.4(2) 6_657 6_657 ?
B1 Gd1 B1 136.3(2) . 6_657 ?
O4 Gd1 K2 51.08(10) . . ?
O5 Gd1 K2 60.49(9) 3_656 . ?
O5 Gd1 K2 119.64(9) 5_656 . ?
O2 Gd1 K2 96.61(10) . . ?
O3 Gd1 K2 47.57(9) . . ?
O1 Gd1 K2 150.09(3) 6_657 . ?
O2 Gd1 K2 121.05(10) 6_657 . ?
B1 Gd1 K2 70.91(15) . . ?
B1 Gd1 K2 142.50(12) 6_657 . ?
O4 Gd1 K2 51.08(10) . 7_565 ?
O5 Gd1 K2 119.64(9) 3_656 7_565 ?
O5 Gd1 K2 60.49(9) 5_656 7_565 ?
O2 Gd1 K2 96.61(10) . 7_565 ?
O3 Gd1 K2 47.57(9) . 7_565 ?
O1 Gd1 K2 150.09(3) 6_657 7_565 ?
O2 Gd1 K2 121.05(10) 6_657 7_565 ?
B1 Gd1 K2 70.91(15) . 7_565 ?
B1 Gd1 K2 142.50(12) 6_657 7_565 ?
K2 Gd1 K2 59.14(4) . 7_565 ?
O4 Gd1 K2 51.61(10) . 5_666 ?
O5 Gd1 K2 59.44(10) 3_656 5_666 ?
O5 Gd1 K2 121.18(10) 5_656 5_666 ?
O2 Gd1 K2 148.77(3) . 5_666 ?
O3 Gd1 K2 120.73(10) . 5_666 ?
O1 Gd1 K2 96.25(11) 6_657 5_666 ?
O2 Gd1 K2 48.13(8) 6_657 5_666 ?
B1 Gd1 K2 141.26(11) . 5_666 ?
B1 Gd1 K2 71.58(17) 6_657 5_666 ?
K2 Gd1 K2 73.33(3) . 5_666 ?
K2 Gd1 K2 102.68(2) 7_565 5_666 ?
O3 K1 O1 52.68(15) . . ?
O3 K1 O5 95.08(14) . 6_556 ?
O1 K1 O5 141.35(12) . 6_556 ?
O3 K1 O5 95.08(14) . 4_455 ?
O1 K1 O5 141.35(13) . 4_455 ?
O5 K1 O5 46.48(15) 6_556 4_455 ?
O3 K1 B1 26.2(2) . . ?
O1 K1 B1 26.49(19) . . ?
O5 K1 B1 118.88(18) 6_556 . ?
O5 K1 B1 118.88(18) 4_455 . ?
O3 K1 O5 140.12(12) . 1_455 ?
O1 K1 O5 93.49(13) . 1_455 ?
O5 K1 O5 104.07(10) 6_556 1_455 ?
O5 K1 O5 123.46(9) 4_455 1_455 ?
B1 K1 O5 117.66(18) . 1_455 ?
O3 K1 O5 140.12(12) . 7_465 ?
O1 K1 O5 93.49(13) . 7_465 ?
O5 K1 O5 123.46(9) 6_556 7_465 ?
O5 K1 O5 104.07(10) 4_455 7_465 ?
B1 K1 O5 117.66(18) . 7_465 ?
O5 K1 O5 45.97(15) 1_455 7_465 ?
O3 K1 B2 107.2(2) . 6_556 ?
O1 K1 B2 159.9(2) . 6_556 ?
O5 K1 B2 25.88(10) 6_556 6_556 ?
O5 K1 B2 25.88(10) 4_455 6_556 ?
B1 K1 B2 133.4(3) . 6_556 ?
O5 K1 B2 104.96(17) 1_455 6_556 ?
O5 K1 B2 104.96(17) 7_465 6_556 ?
O3 K1 B2 134.7(2) . 1_455 ?
O1 K1 B2 82.1(2) . 1_455 ?
O5 K1 B2 125.97(17) 6_556 1_455 ?
O5 K1 B2 125.97(17) 4_455 1_455 ?
B1 K1 B2 108.6(2) . 1_455 ?
O5 K1 B2 25.66(10) 1_455 1_455 ?
O5 K1 B2 25.66(10) 7_465 1_455 ?
B2 K1 B2 118.0(2) 6_556 1_455 ?
O3 K1 B1 90.04(16) . 5_556 ?
O1 K1 B1 89.46(15) . 5_556 ?
O5 K1 B1 67.46(16) 6_556 5_556 ?
O5 K1 B1 113.94(17) 4_455 5_556 ?
B1 K1 B1 89.72(16) . 5_556 ?
O5 K1 B1 66.59(17) 1_455 5_556 ?
O5 K1 B1 112.56(18) 7_465 5_556 ?
B2 K1 B1 90.66(15) 6_556 5_556 ?
B2 K1 B1 89.47(16) 1_455 5_556 ?
O3 K1 B1 90.04(16) . 5_566 ?
O1 K1 B1 89.46(15) . 5_566 ?
O5 K1 B1 113.94(17) 6_556 5_566 ?
O5 K1 B1 67.46(16) 4_455 5_566 ?
B1 K1 B1 89.72(16) . 5_566 ?
O5 K1 B1 112.56(18) 1_455 5_566 ?
O5 K1 B1 66.59(17) 7_465 5_566 ?
B2 K1 B1 90.66(15) 6_556 5_566 ?
B2 K1 B1 89.47(16) 1_455 5_566 ?
B1 K1 B1 178.6(3) 5_556 5_566 ?
O3 K1 K2 44.48(9) . . ?
O1 K1 K2 88.94(11) . . ?
O5 K1 K2 76.81(9) 6_556 . ?
O5 K1 K2 53.26(8) 4_455 . ?
B1 K1 K2 65.76(16) . . ?
O5 K1 K2 174.51(8) 1_455 . ?
O5 K1 K2 129.00(8) 7_465 . ?
B2 K1 K2 73.39(16) 6_556 . ?
B2 K1 K2 150.71(6) 1_455 . ?
B1 K1 K2 118.40(17) 5_556 . ?
B1 K1 K2 62.50(16) 5_566 . ?
O3 K2 O2 166.37(16) . 2_564 ?
O3 K2 O1 99.16(14) . 5_566 ?
O2 K2 O1 70.46(14) 2_564 5_566 ?
O3 K2 O4 72.26(15) . . ?
O2 K2 O4 120.02(14) 2_564 . ?
O1 K2 O4 163.25(16) 5_566 . ?
O3 K2 O4 119.04(15) . 5_666 ?
O2 K2 O4 71.23(13) 2_564 5_666 ?
O1 K2 O4 91.95(12) 5_566 5_666 ?
O4 K2 O4 80.40(4) . 5_666 ?
O3 K2 O5 97.31(14) . 4_455 ?
O2 K2 O5 71.38(12) 2_564 4_455 ?
O1 K2 O5 71.66(13) 5_566 4_455 ?
O4 K2 O5 122.93(12) . 4_455 ?
O4 K2 O5 142.37(12) 5_666 4_455 ?
O3 K2 O5 119.10(13) . 7_565 ?
O2 K2 O5 72.06(12) 2_564 7_565 ?
O1 K2 O5 141.68(13) 5_566 7_565 ?
O4 K2 O5 48.34(12) . 7_565 ?
O4 K2 O5 68.51(12) 5_666 7_565 ?
O5 K2 O5 103.50(7) 4_455 7_565 ?
O3 K2 O5 71.47(13) . 3_656 ?
O2 K2 O5 117.28(12) 2_564 3_656 ?
O1 K2 O5 95.38(14) 5_566 3_656 ?
O4 K2 O5 68.43(12) . 3_656 ?
O4 K2 O5 47.79(12) 5_666 3_656 ?
O5 K2 O5 161.70(7) 4_455 3_656 ?
O5 K2 O5 94.67(10) 7_565 3_656 ?
O3 K2 B2 93.45(16) . . ?
O2 K2 B2 96.90(16) 2_564 . ?
O1 K2 B2 167.33(17) 5_566 . ?
O4 K2 B2 26.45(19) . . ?
O4 K2 B2 82.95(15) 5_666 . ?
O5 K2 B2 105.63(18) 4_455 . ?
O5 K2 B2 25.88(13) 7_565 . ?
O5 K2 B2 89.78(19) 3_656 . ?
O3 K2 B2 95.86(17) . 5_666 ?
O2 K2 B2 91.87(15) 2_564 5_666 ?
O1 K2 B2 84.03(16) 5_566 5_666 ?
O4 K2 B2 82.64(15) . 5_666 ?
O4 K2 B2 26.04(18) 5_666 5_666 ?
O5 K2 B2 153.87(14) 4_455 5_666 ?
O5 K2 B2 89.51(18) 7_565 5_666 ?
O5 K2 B2 25.56(13) 3_656 5_666 ?
B2 K2 B2 95.98(15) . 5_666 ?
O3 K2 K2 48.05(8) . 7_565 ?
O2 K2 K2 133.52(8) 2_564 7_565 ?
O1 K2 K2 133.34(8) 5_566 7_565 ?
O4 K2 K2 50.68(7) . 7_565 ?
O4 K2 K2 130.83(7) 5_666 7_565 ?
O5 K2 K2 80.14(8) 4_455 7_565 ?
O5 K2 K2 80.16(8) 7_565 7_565 ?
O5 K2 K2 101.18(8) 3_656 7_565 ?
B2 K2 K2 56.23(10) . 7_565 ?
B2 K2 K2 124.91(10) 5_666 7_565 ?
O3 K2 Gd1 43.58(12) . . ?
O2 K2 Gd1 149.66(11) 2_564 . ?
O1 K2 Gd1 122.83(12) 5_566 . ?
O4 K2 Gd1 41.44(11) . . ?
O4 K2 Gd1 80.65(9) 5_666 . ?
O5 K2 Gd1 136.80(8) 4_455 . ?
O5 K2 Gd1 87.42(8) 7_565 . ?
O5 K2 Gd1 40.75(8) 3_656 . ?
B2 K2 Gd1 67.90(16) . . ?
B2 K2 Gd1 65.19(10) 5_666 . ?
K2 K2 Gd1 60.43(2) 7_565 . ?
B1 O1 Gd1 92.8(4) . 6_557 ?
B1 O1 K2 136.65(8) . 3_546 ?
Gd1 O1 K2 88.72(15) 6_557 3_546 ?
B1 O1 K2 136.65(8) . 5_566 ?
Gd1 O1 K2 88.72(15) 6_557 5_566 ?
K2 O1 K2 86.68(16) 3_546 5_566 ?
B1 O1 K1 90.0(4) . . ?
Gd1 O1 K1 177.2(2) 6_557 . ?
K2 O1 K1 89.24(14) 3_546 . ?
K2 O1 K1 89.24(14) 5_566 . ?
B1 O2 Gd1 91.7(4) . . ?
B1 O2 Gd1 91.8(4) . 6_557 ?
Gd1 O2 Gd1 176.5(2) . 6_557 ?
B1 O2 K2 136.47(8) . 2_565 ?
Gd1 O2 K2 89.19(13) . 2_565 ?
Gd1 O2 K2 88.24(13) 6_557 2_565 ?
B1 O2 K2 136.47(8) . 8_656 ?
Gd1 O2 K2 89.19(13) . 8_656 ?
Gd1 O2 K2 88.24(13) 6_557 8_656 ?
K2 O2 K2 87.05(15) 2_565 8_656 ?
B1 O3 Gd1 92.4(5) . . ?
B1 O3 K2 138.04(8) . . ?
Gd1 O3 K2 88.86(15) . . ?
B1 O3 K2 138.04(8) . 7_565 ?
Gd1 O3 K2 88.86(15) . 7_565 ?
K2 O3 K2 83.91(16) . 7_565 ?
B1 O3 K1 91.8(5) . . ?
Gd1 O3 K1 175.8(2) . . ?
K2 O3 K1 88.04(14) . . ?
K2 O3 K1 88.04(14) 7_565 . ?
B2 O4 Gd1 179.7(5) . . ?
B2 O4 K2 92.3(4) . 7_565 ?
Gd1 O4 K2 87.47(14) . 7_565 ?
B2 O4 K2 92.3(4) . . ?
Gd1 O4 K2 87.47(14) . . ?
K2 O4 K2 78.64(15) 7_565 . ?
B2 O4 K2 93.0(3) . 5_666 ?
Gd1 O4 K2 87.18(14) . 5_666 ?
K2 O4 K2 174.4(2) 7_565 5_666 ?
K2 O4 K2 99.60(4) . 5_666 ?
B2 O4 K2 93.0(3) . 3_646 ?
Gd1 O4 K2 87.18(14) . 3_646 ?
K2 O4 K2 99.60(4) 7_565 3_646 ?
K2 O4 K2 174.4(2) . 3_646 ?
K2 O4 K2 81.65(15) 5_666 3_646 ?
B2 O5 Gd1 149.9(4) . 5_656 ?
B2 O5 K1 80.4(4) . 6_656 ?
Gd1 O5 K1 113.17(14) 5_656 6_656 ?
B2 O5 K2 129.7(4) . 4 ?
Gd1 O5 K2 80.40(11) 5_656 4 ?
K1 O5 K2 74.11(9) 6_656 4 ?
B2 O5 K2 78.3(4) . 7_565 ?
Gd1 O5 K2 79.85(11) 5_656 7_565 ?
K1 O5 K2 74.52(10) 6_656 7_565 ?
K2 O5 K2 132.15(14) 4 7_565 ?
B2 O5 K1 80.2(4) . 1_655 ?
Gd1 O5 K1 113.25(14) 5_656 1_655 ?
K1 O5 K1 116.91(12) 6_656 1_655 ?
K2 O5 K1 74.13(9) 4 1_655 ?
K2 O5 K1 153.44(14) 7_565 1_655 ?
B2 O5 K2 79.1(4) . 3_646 ?
Gd1 O5 K2 78.76(11) 5_656 3_646 ?
K1 O5 K2 153.70(14) 6_656 3_646 ?
K2 O5 K2 132.07(13) 4 3_646 ?
K2 O5 K2 85.33(10) 7_565 3_646 ?
K1 O5 K2 75.40(10) 1_655 3_646 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O3 B1 O1 Gd1 180.000(2) . . . 6_557 ?
O2 B1 O1 Gd1 0.000(2) . . . 6_557 ?
K1 B1 O1 Gd1 180.000(1) . . . 6_557 ?
K1 B1 O1 Gd1 -89.46(15) 5_566 . . 6_557 ?
K1 B1 O1 Gd1 89.46(15) 5_556 . . 6_557 ?
O3 B1 O1 K2 88.9(6) . . . 3_546 ?
O2 B1 O1 K2 -91.1(6) . . . 3_546 ?
Gd1 B1 O1 K2 -91.1(6) 6_557 . . 3_546 ?
K1 B1 O1 K2 88.9(6) . . . 3_546 ?
K1 B1 O1 K2 179.4(5) 5_566 . . 3_546 ?
K1 B1 O1 K2 -1.6(7) 5_556 . . 3_546 ?
O3 B1 O1 K2 -88.9(6) . . . 5_566 ?
O2 B1 O1 K2 91.1(6) . . . 5_566 ?
Gd1 B1 O1 K2 91.1(6) 6_557 . . 5_566 ?
K1 B1 O1 K2 -88.9(6) . . . 5_566 ?
K1 B1 O1 K2 1.6(7) 5_566 . . 5_566 ?
K1 B1 O1 K2 -179.4(5) 5_556 . . 5_566 ?
O3 B1 O1 K1 0.000(2) . . . . ?
O2 B1 O1 K1 180.000(2) . . . . ?
Gd1 B1 O1 K1 180.000(1) 6_557 . . . ?
K1 B1 O1 K1 90.54(15) 5_566 . . . ?
K1 B1 O1 K1 -90.54(15) 5_556 . . . ?
O3 B1 O2 Gd1 0.000(1) . . . . ?
O1 B1 O2 Gd1 180.000(1) . . . . ?
Gd1 B1 O2 Gd1 180.000(1) 6_557 . . . ?
K1 B1 O2 Gd1 -90.66(15) 5_566 . . . ?
K1 B1 O2 Gd1 90.66(15) 5_556 . . . ?
O3 B1 O2 Gd1 180.000(1) . . . 6_557 ?
O1 B1 O2 Gd1 0.000(1) . . . 6_557 ?
Gd1 B1 O2 Gd1 180.000(1) . . . 6_557 ?
K1 B1 O2 Gd1 89.34(15) 5_566 . . 6_557 ?
K1 B1 O2 Gd1 -89.34(15) 5_556 . . 6_557 ?
O3 B1 O2 K2 90.6(5) . . . 2_565 ?
O1 B1 O2 K2 -89.4(5) . . . 2_565 ?
Gd1 B1 O2 K2 90.6(5) . . . 2_565 ?
Gd1 B1 O2 K2 -89.4(5) 6_557 . . 2_565 ?
K1 B1 O2 K2 0.0(7) 5_566 . . 2_565 ?
K1 B1 O2 K2 -178.7(4) 5_556 . . 2_565 ?
O3 B1 O2 K2 -90.6(5) . . . 8_656 ?
O1 B1 O2 K2 89.4(5) . . . 8_656 ?
Gd1 B1 O2 K2 -90.6(5) . . . 8_656 ?
Gd1 B1 O2 K2 89.4(5) 6_557 . . 8_656 ?
K1 B1 O2 K2 178.7(4) 5_566 . . 8_656 ?
K1 B1 O2 K2 0.0(7) 5_556 . . 8_656 ?
O1 B1 O3 Gd1 180.000(2) . . . . ?
O2 B1 O3 Gd1 0.000(2) . . . . ?
K1 B1 O3 Gd1 180.000(1) . . . . ?
K1 B1 O3 Gd1 90.06(17) 5_566 . . . ?
K1 B1 O3 Gd1 -90.06(17) 5_556 . . . ?
O1 B1 O3 K2 89.1(6) . . . . ?
O2 B1 O3 K2 -90.9(6) . . . . ?
Gd1 B1 O3 K2 -90.9(6) . . . . ?
K1 B1 O3 K2 89.1(6) . . . . ?
K1 B1 O3 K2 -0.8(8) 5_566 . . . ?
K1 B1 O3 K2 179.0(5) 5_556 . . . ?
O1 B1 O3 K2 -89.1(6) . . . 7_565 ?
O2 B1 O3 K2 90.9(6) . . . 7_565 ?
Gd1 B1 O3 K2 90.9(6) . . . 7_565 ?
K1 B1 O3 K2 -89.1(6) . . . 7_565 ?
K1 B1 O3 K2 -179.0(5) 5_566 . . 7_565 ?
K1 B1 O3 K2 0.9(8) 5_556 . . 7_565 ?
O1 B1 O3 K1 0.000(2) . . . . ?
O2 B1 O3 K1 180.000(2) . . . . ?
Gd1 B1 O3 K1 180.000(1) . . . . ?
K1 B1 O3 K1 -89.94(17) 5_566 . . . ?
K1 B1 O3 K1 89.94(17) 5_556 . . . ?
O5 B2 O4 K2 -50.4(7) . . . 7_565 ?
O5 B2 O4 K2 129.1(7) 7_565 . . 7_565 ?
K2 B2 O4 K2 78.72(16) . . . 7_565 ?
K1 B2 O4 K2 39.36(8) 6_656 . . 7_565 ?
K2 B2 O4 K2 178.46(16) 5_666 . . 7_565 ?
K2 B2 O4 K2 -99.74(4) 3_646 . . 7_565 ?
K1 B2 O4 K2 -140.64(8) 1_655 . . 7_565 ?
O5 B2 O4 K2 -129.1(7) . . . . ?
O5 B2 O4 K2 50.4(7) 7_565 . . . ?
K2 B2 O4 K2 -78.72(16) 7_565 . . . ?
K1 B2 O4 K2 -39.36(8) 6_656 . . . ?
K2 B2 O4 K2 99.74(4) 5_666 . . . ?
K2 B2 O4 K2 -178.46(16) 3_646 . . . ?
K1 B2 O4 K2 140.64(8) 1_655 . . . ?
O5 B2 O4 K2 131.1(7) . . . 5_666 ?
O5 B2 O4 K2 -49.3(7) 7_565 . . 5_666 ?
K2 B2 O4 K2 -178.46(16) 7_565 . . 5_666 ?
K2 B2 O4 K2 -99.74(4) . . . 5_666 ?
K1 B2 O4 K2 -139.10(8) 6_656 . . 5_666 ?
K2 B2 O4 K2 81.79(17) 3_646 . . 5_666 ?
K1 B2 O4 K2 40.90(8) 1_655 . . 5_666 ?
O5 B2 O4 K2 49.3(7) . . . 3_646 ?
O5 B2 O4 K2 -131.1(7) 7_565 . . 3_646 ?
K2 B2 O4 K2 99.74(4) 7_565 . . 3_646 ?
K2 B2 O4 K2 178.46(16) . . . 3_646 ?
K1 B2 O4 K2 139.10(8) 6_656 . . 3_646 ?
K2 B2 O4 K2 -81.79(16) 5_666 . . 3_646 ?
K1 B2 O4 K2 -40.90(8) 1_655 . . 3_646 ?
O5 B2 O5 Gd1 -179.64(19) 7_565 . . 5_656 ?
O4 B2 O5 Gd1 -0.1(15) . . . 5_656 ?
K2 B2 O5 Gd1 -44.3(9) 7_565 . . 5_656 ?
K2 B2 O5 Gd1 -78.3(11) . . . 5_656 ?
K1 B2 O5 Gd1 -120.3(8) 6_656 . . 5_656 ?
K2 B2 O5 Gd1 78.2(11) 5_666 . . 5_656 ?
K2 B2 O5 Gd1 43.1(8) 3_646 . . 5_656 ?
K1 B2 O5 Gd1 120.0(8) 1_655 . . 5_656 ?
O5 B2 O5 K1 -59.3(7) 7_565 . . 6_656 ?
O4 B2 O5 K1 120.2(7) . . . 6_656 ?
K2 B2 O5 K1 76.03(11) 7_565 . . 6_656 ?
K2 B2 O5 K1 42.0(5) . . . 6_656 ?
K2 B2 O5 K1 -161.5(7) 5_666 . . 6_656 ?
K2 B2 O5 K1 163.45(16) 3_646 . . 6_656 ?
K1 B2 O5 K1 -119.67(13) 1_655 . . 6_656 ?
O5 B2 O5 K2 0.6(11) 7_565 . . 4 ?
O4 B2 O5 K2 -179.9(4) . . . 4 ?
K2 B2 O5 K2 136.0(4) 7_565 . . 4 ?
K2 B2 O5 K2 102.0(6) . . . 4 ?
K1 B2 O5 K2 60.0(4) 6_656 . . 4 ?
K2 B2 O5 K2 -101.5(6) 5_666 . . 4 ?
K2 B2 O5 K2 -136.6(4) 3_646 . . 4 ?
K1 B2 O5 K2 -59.7(4) 1_655 . . 4 ?
O5 B2 O5 K2 -135.3(8) 7_565 . . 7_565 ?
O4 B2 O5 K2 44.2(7) . . . 7_565 ?
K2 B2 O5 K2 -34.0(5) . . . 7_565 ?
K1 B2 O5 K2 -76.03(11) 6_656 . . 7_565 ?
K2 B2 O5 K2 122.5(6) 5_666 . . 7_565 ?
K2 B2 O5 K2 87.43(12) 3_646 . . 7_565 ?
K1 B2 O5 K2 164.30(16) 1_655 . . 7_565 ?
O5 B2 O5 K1 60.4(7) 7_565 . . 1_655 ?
O4 B2 O5 K1 -120.1(7) . . . 1_655 ?
K2 B2 O5 K1 -164.30(16) 7_565 . . 1_655 ?
K2 B2 O5 K1 161.7(6) . . . 1_655 ?
K1 B2 O5 K1 119.67(13) 6_656 . . 1_655 ?
K2 B2 O5 K1 -41.8(6) 5_666 . . 1_655 ?
K2 B2 O5 K1 -76.87(11) 3_646 . . 1_655 ?
O5 B2 O5 K2 137.2(8) 7_565 . . 3_646 ?
O4 B2 O5 K2 -43.3(7) . . . 3_646 ?
K2 B2 O5 K2 -87.43(11) 7_565 . . 3_646 ?
K2 B2 O5 K2 -121.4(6) . . . 3_646 ?
K1 B2 O5 K2 -163.45(16) 6_656 . . 3_646 ?
K2 B2 O5 K2 35.1(6) 5_666 . . 3_646 ?
K1 B2 O5 K2 76.87(11) 1_655 . . 3_646 ?

_refine_diff_density_max         1.745
_refine_diff_density_min         -2.276
_refine_diff_density_rms         0.379



